# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_1

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Gd4 H12 O24 S4'
_chemical_formula_sum            'Gd4 H12 O24 S4'
_chemical_formula_weight         1153.34

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   'P 21 21 21'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'

_cell_length_a                   10.743(2)
_cell_length_b                   10.981(2)
_cell_length_c                   16.751(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     1976.1(7)
_cell_formula_units_Z            4
_cell_measurement_temperature    113(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.13
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.877
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2096
_exptl_absorpt_coefficient_mu    13.788
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.079
_exptl_absorpt_correction_T_max  0.167
_exptl_absorpt_process_details   CrystalClear

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      113(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_monochromator  Confocal
_diffrn_radiation_detector       CCD
_diffrn_measurement_device       
;
Saturn70 (4x4 bin mode)
;
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            19551
_diffrn_reflns_av_R_equivalents  0.0386
_diffrn_reflns_av_sigmaI/netI    0.0339
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         2.22
_diffrn_reflns_theta_max         27.89
_reflns_number_total             4688
_reflns_number_gt                4268
_reflns_threshold_expression     >2sigma(I)


_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0261P)²+0.4208P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00281(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.360(12)
_refine_ls_number_reflns         4688
_refine_ls_number_parameters     291
_refine_ls_number_restraints     196
_refine_ls_R_factor_all          0.0235
_refine_ls_R_factor_gt           0.0215
_refine_ls_wR_factor_ref         0.0565
_refine_ls_wR_factor_gt          0.0561
_refine_ls_goodness_of_fit_ref   1.112
_refine_ls_restrained_S_all      1.128
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Gd1 Gd 0.05942(2) 0.49596(2) 0.803454(14) 0.00564(7) Uani 1 1 d U . .
Gd2 Gd 0.42604(2) 0.50958(3) 0.791930(15) 0.00743(7) Uani 1 1 d U . .
Gd3 Gd 0.26664(3) 0.31995(2) 0.952170(18) 0.00609(7) Uani 1 1 d U . .
Gd4 Gd 0.24919(2) 0.67951(3) 0.954922(18) 0.00629(7) Uani 1 1 d U . .
O1 O 0.3982(4) 0.3262(4) 0.5563(3) 0.0193(9) Uani 1 1 d U . .
O2 O 0.5997(4) 0.3060(3) 0.6149(3) 0.0179(9) Uani 1 1 d U . .
O3 O 0.4227(4) 0.3612(4) 0.6946(3) 0.0209(10) Uani 1 1 d U . .
O4 O 0.5594(4) 0.6580(3) 0.8564(3) 0.0176(9) Uani 1 1 d U . .
O5 O 0.3652(4) 0.7171(4) 0.5616(3) 0.0232(10) Uani 1 1 d U . .
O6 O 0.3977(4) 0.8813(4) 0.6561(3) 0.0232(10) Uani 1 1 d U . .
O7 O 0.3904(4) 0.6700(4) 0.6996(3) 0.0218(10) Uani 1 1 d U . .
O8 O 0.4361(4) 0.2445(4) 0.8747(3) 0.0206(10) Uani 1 1 d U . .
O9 O 0.0850(4) 0.6476(3) 0.5551(3) 0.0161(9) Uani 1 1 d U . .
O10 O 0.0448(4) 0.6282(4) 0.6948(3) 0.0194(10) Uani 1 1 d U . .
O11 O -0.0360(4) 0.3247(3) 0.8675(3) 0.0150(9) Uani 1 1 d U . .
O12 O 0.1249(4) 0.1780(4) 0.8935(3) 0.0187(10) Uani 1 1 d U . .
O13 O 0.3963(4) 0.6561(3) 1.0578(3) 0.0181(10) Uani 1 1 d U . .
O14 O 0.4445(4) 0.6428(3) 1.1969(3) 0.0176(9) Uani 1 1 d U . .
O15 O 0.6109(4) 0.6721(4) 1.1009(3) 0.0204(10) Uani 1 1 d U . .
O16 O -0.0361(4) 0.6656(3) 0.8724(3) 0.0169(9) Uani 1 1 d U . .
O17 O 0.1324(3) 0.4921(3) 0.9438(2) 0.0099(7) Uani 1 1 d DU . .
H17 H 0.0731 0.4950 0.9776 0.012 Uiso 1 1 d RD . .
O18 O 0.3804(3) 0.5049(3) 0.92803(19) 0.0077(7) Uani 1 1 d DU . .
H18 H 0.4332 0.4988 0.9654 0.009 Uiso 1 1 d RD . .
O19 O 0.2364(3) 0.6224(3) 0.8198(2) 0.0080(8) Uani 1 1 d DU . .
H19 H 0.2446 0.6887 0.7937 0.010 Uiso 1 1 d RD . .
O20 O 0.2453(3) 0.3836(3) 0.8145(2) 0.0068(8) Uani 1 1 d DU . .
H20 H 0.2495 0.3154 0.7915 0.008 Uiso 1 1 d RD . .
O1W O -0.1649(4) 0.4881(4) 0.7838(3) 0.0353(12) Uani 1 1 d U . .
O2W O 0.6184(4) 0.5317(4) 0.7012(3) 0.0229(10) Uani 1 1 d U . .
O3W O 0.3289(4) 0.1144(4) 0.9962(3) 0.0254(11) Uani 1 1 d U . .
O4W O 0.2611(4) 0.8810(4) 1.0342(3) 0.0188(10) Uani 1 1 d U . .
S1 S 0.46547(13) 0.28789(12) 0.62712(8) 0.0084(3) Uani 1 1 d U . .
S2 S 0.42704(13) 0.75255(12) 0.63482(9) 0.0105(3) Uani 1 1 d U . .
S3 S 0.01015(13) 0.69284(12) 0.62246(9) 0.0092(3) Uani 1 1 d U . .
S4 S 0.47948(13) 0.69976(12) 1.12128(9) 0.0093(3) Uani 1 1 d U . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Gd1 O10 2.334(5) . ?
Gd1 O14 2.347(4) 2_564 ?
Gd1 O20 2.355(3) . ?
Gd1 O19 2.371(4) . ?
Gd1 O11 2.395(4) . ?
Gd1 O16 2.420(4) . ?
Gd1 O1W 2.433(4) . ?
Gd1 O17 2.479(3) . ?
Gd1 Gd4 3.8284(6) . ?
Gd1 Gd3 3.8596(6) . ?
Gd1 Gd2 3.9461(9) . ?
Gd2 O3 2.305(4) . ?
Gd2 O18 2.333(3) . ?
Gd2 O7 2.376(4) . ?
Gd2 O20 2.413(4) . ?
Gd2 O4 2.423(4) . ?
Gd2 O19 2.430(4) . ?
Gd2 O6 2.515(4) 3_646 ?
Gd2 O2W 2.576(4) . ?
Gd2 Gd3 3.8044(6) . ?
Gd2 Gd4 3.8139(6) . ?
Gd3 O5 2.352(5) 2_565 ?
Gd3 O9 2.375(4) 2_565 ?
Gd3 O17 2.381(4) . ?
Gd3 O8 2.384(4) . ?
Gd3 O12 2.390(4) . ?
Gd3 O18 2.404(4) . ?
Gd3 O20 2.421(4) . ?
Gd3 O3W 2.467(4) . ?
Gd3 Gd4 3.9530(9) . ?
Gd4 O1 2.322(4) 2_565 ?
Gd4 O19 2.352(4) . ?
Gd4 O13 2.353(4) . ?
Gd4 O15 2.395(4) 4_467 ?
Gd4 O17 2.417(4) . ?
Gd4 O18 2.422(4) . ?
Gd4 O2 2.436(4) 3_656 ?
Gd4 O4W 2.583(5) . ?
O1 S1 1.452(4) . ?
O1 Gd4 2.322(4) 2_564 ?
O2 S1 1.470(4) . ?
O2 Gd4 2.436(4) 3_646 ?
O3 S1 1.462(5) . ?
O4 S1 1.477(4) 3_656 ?
O5 S2 1.448(5) . ?
O5 Gd3 2.352(4) 2_564 ?
O6 S2 1.492(4) . ?
O6 Gd2 2.515(4) 3_656 ?
O7 S2 1.467(4) . ?
O8 S2 1.482(4) 3_646 ?
O9 S3 1.472(5) . ?
O9 Gd3 2.375(4) 2_564 ?
O10 S3 1.453(5) . ?
O11 S3 1.484(4) 3_546 ?
O12 S3 1.484(4) 3_546 ?
O13 S4 1.469(5) . ?
O14 S4 1.462(5) . ?
O14 Gd1 2.347(4) 2_565 ?
O15 S4 1.484(5) . ?
O15 Gd4 2.395(4) 4_567 ?
O16 S4 1.492(4) 4_467 ?
S1 O4 1.477(4) 3_646 ?
S2 O8 1.482(5) 3_656 ?
S3 O11 1.484(4) 3_556 ?
S3 O12 1.484(4) 3_556 ?
S4 O16 1.492(4) 4_567 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O10 Gd1 O14 79.01(13) . 2_564 ?
O10 Gd1 O20 116.35(14) . . ?
O14 Gd1 O20 74.62(14) 2_564 . ?
O10 Gd1 O19 77.27(14) . . ?
O14 Gd1 O19 118.86(14) 2_564 . ?
O20 Gd1 O19 67.52(12) . . ?
O10 Gd1 O11 144.01(15) . . ?
O14 Gd1 O11 79.82(15) 2_564 . ?
O20 Gd1 O11 85.20(13) . . ?
O19 Gd1 O11 138.70(14) . . ?
O10 Gd1 O16 82.25(15) . . ?
O14 Gd1 O16 148.73(15) 2_564 . ?
O20 Gd1 O16 136.53(14) . . ?
O19 Gd1 O16 80.46(13) . . ?
O11 Gd1 O16 102.06(12) . . ?
O10 Gd1 O1W 81.37(16) . . ?
O14 Gd1 O1W 81.72(16) 2_564 . ?
O20 Gd1 O1W 146.28(15) . . ?
O19 Gd1 O1W 146.17(14) . . ?
O11 Gd1 O1W 67.00(16) . . ?
O16 Gd1 O1W 70.85(15) . . ?
O10 Gd1 O17 140.51(13) . . ?
O14 Gd1 O17 135.72(13) 2_564 . ?
O20 Gd1 O17 69.41(13) . . ?
O19 Gd1 O17 69.30(13) . . ?
O11 Gd1 O17 72.37(13) . . ?
O16 Gd1 O17 72.23(13) . . ?
O1W Gd1 O17 116.19(15) . . ?
O10 Gd1 Gd4 103.02(10) . . ?
O14 Gd1 Gd4 148.80(10) 2_564 . ?
O20 Gd1 Gd4 76.84(9) . . ?
O19 Gd1 Gd4 35.69(10) . . ?
O11 Gd1 Gd4 110.14(10) . . ?
O16 Gd1 Gd4 60.30(10) . . ?
O1W Gd1 Gd4 129.48(12) . . ?
O17 Gd1 Gd4 37.99(8) . . ?
O10 Gd1 Gd3 148.62(11) . . ?
O14 Gd1 Gd3 100.15(10) 2_564 . ?
O20 Gd1 Gd3 36.67(10) . . ?
O19 Gd1 Gd3 75.88(9) . . ?
O11 Gd1 Gd3 64.18(10) . . ?
O16 Gd1 Gd3 108.79(10) . . ?
O1W Gd1 Gd3 129.85(12) . . ?
O17 Gd1 Gd3 36.56(8) . . ?
Gd4 Gd1 Gd3 61.884(14) . . ?
O10 Gd1 Gd2 90.30(10) . . ?
O14 Gd1 Gd2 90.31(10) 2_564 . ?
O20 Gd1 Gd2 34.63(9) . . ?
O19 Gd1 Gd2 35.20(9) . . ?
O11 Gd1 Gd2 118.59(10) . . ?
O16 Gd1 Gd2 114.69(10) . . ?
O1W Gd1 Gd2 169.41(12) . . ?
O17 Gd1 Gd2 74.40(8) . . ?
Gd4 Gd1 Gd2 58.733(9) . . ?
Gd3 Gd1 Gd2 58.325(10) . . ?
O3 Gd2 O18 132.25(14) . . ?
O3 Gd2 O7 93.51(14) . . ?
O18 Gd2 O7 128.24(14) . . ?
O3 Gd2 O20 72.12(14) . . ?
O18 Gd2 O20 70.45(13) . . ?
O7 Gd2 O20 113.41(13) . . ?
O3 Gd2 O4 143.09(15) . . ?
O18 Gd2 O4 72.77(13) . . ?
O7 Gd2 O4 83.48(14) . . ?
O20 Gd2 O4 142.30(14) . . ?
O3 Gd2 O19 118.92(14) . . ?
O18 Gd2 O19 69.32(13) . . ?
O7 Gd2 O19 67.17(14) . . ?
O20 Gd2 O19 65.66(12) . . ?
O4 Gd2 O19 93.83(13) . . ?
O3 Gd2 O6 81.98(15) . 3_646 ?
O18 Gd2 O6 78.93(13) . 3_646 ?
O7 Gd2 O6 139.63(14) . 3_646 ?
O20 Gd2 O6 103.33(13) . 3_646 ?
O4 Gd2 O6 77.15(14) . 3_646 ?
O19 Gd2 O6 148.24(14) . 3_646 ?
O3 Gd2 O2W 70.26(14) . . ?
O18 Gd2 O2W 138.34(13) . . ?
O7 Gd2 O2W 71.04(14) . . ?
O20 Gd2 O2W 142.33(13) . . ?
O4 Gd2 O2W 74.04(14) . . ?
O19 Gd2 O2W 137.53(13) . . ?
O6 Gd2 O2W 69.70(14) 3_646 . ?
O3 Gd2 Gd3 96.03(11) . . ?
O18 Gd2 Gd3 37.22(9) . . ?
O7 Gd2 Gd3 142.46(10) . . ?
O20 Gd2 Gd3 38.18(9) . . ?
O4 Gd2 Gd3 108.65(11) . . ?
O19 Gd2 Gd3 76.48(9) . . ?
O6 Gd2 Gd3 77.77(10) 3_646 . ?
O2W Gd2 Gd3 145.97(9) . . ?
O3 Gd2 Gd4 147.61(11) . . ?
O18 Gd2 Gd4 37.46(9) . . ?
O7 Gd2 Gd4 91.33(11) . . ?
O20 Gd2 Gd4 76.57(9) . . ?
O4 Gd2 Gd4 69.30(10) . . ?
O19 Gd2 Gd4 36.41(9) . . ?
O6 Gd2 Gd4 113.66(11) 3_646 . ?
O2W Gd2 Gd4 140.85(9) . . ?
Gd3 Gd2 Gd4 62.515(14) . . ?
O3 Gd2 Gd1 89.56(11) . . ?
O18 Gd2 Gd1 75.01(8) . . ?
O7 Gd2 Gd1 84.22(10) . . ?
O20 Gd2 Gd1 33.67(8) . . ?
O4 Gd2 Gd1 126.41(10) . . ?
O19 Gd2 Gd1 34.22(9) . . ?
O6 Gd2 Gd1 135.50(10) 3_646 . ?
O2W Gd2 Gd1 146.41(10) . . ?
Gd3 Gd2 Gd1 59.700(8) . . ?
Gd4 Gd2 Gd1 59.092(9) . . ?
O5 Gd3 O9 82.19(15) 2_565 2_565 ?
O5 Gd3 O17 79.56(13) 2_565 . ?
O9 Gd3 O17 109.25(12) 2_565 . ?
O5 Gd3 O8 145.47(15) 2_565 . ?
O9 Gd3 O8 86.27(15) 2_565 . ?
O17 Gd3 O8 134.91(13) . . ?
O5 Gd3 O12 79.89(16) 2_565 . ?
O9 Gd3 O12 145.49(14) 2_565 . ?
O17 Gd3 O12 96.18(13) . . ?
O8 Gd3 O12 92.05(15) . . ?
O5 Gd3 O18 125.67(13) 2_565 . ?
O9 Gd3 O18 69.77(12) 2_565 . ?
O17 Gd3 O18 68.11(13) . . ?
O8 Gd3 O18 79.29(13) . . ?
O12 Gd3 O18 143.63(13) . . ?
O5 Gd3 O20 137.36(13) 2_565 . ?
O9 Gd3 O20 135.38(13) 2_565 . ?
O17 Gd3 O20 69.96(11) . . ?
O8 Gd3 O20 69.76(13) . . ?
O12 Gd3 O20 74.70(14) . . ?
O18 Gd3 O20 69.14(12) . . ?
O5 Gd3 O3W 76.81(15) 2_565 . ?
O9 Gd3 O3W 74.84(13) 2_565 . ?
O17 Gd3 O3W 155.22(14) . . ?
O8 Gd3 O3W 68.77(15) . . ?
O12 Gd3 O3W 72.49(14) . . ?
O18 Gd3 O3W 133.28(14) . . ?
O20 Gd3 O3W 125.08(14) . . ?
O5 Gd3 Gd2 156.30(10) 2_565 . ?
O9 Gd3 Gd2 97.35(10) 2_565 . ?
O17 Gd3 Gd2 78.25(8) . . ?
O8 Gd3 Gd2 57.49(10) . . ?
O12 Gd3 Gd2 110.69(11) . . ?
O18 Gd3 Gd2 35.93(8) . . ?
O20 Gd3 Gd2 38.03(8) . . ?
O3W Gd3 Gd2 126.15(11) . . ?
O5 Gd3 Gd1 104.03(10) 2_565 . ?
O9 Gd3 Gd1 141.30(9) 2_565 . ?
O17 Gd3 Gd1 38.31(8) . . ?
O8 Gd3 Gd1 105.25(11) . . ?
O12 Gd3 Gd1 72.16(11) . . ?
O18 Gd3 Gd1 76.20(8) . . ?
O20 Gd3 Gd1 35.51(8) . . ?
O3W Gd3 Gd1 143.85(11) . . ?
Gd2 Gd3 Gd1 61.975(14) . . ?
O5 Gd3 Gd4 97.76(10) 2_565 . ?
O9 Gd3 Gd4 82.72(9) 2_565 . ?
O17 Gd3 Gd4 34.83(8) . . ?
O8 Gd3 Gd4 112.94(10) . . ?
O12 Gd3 Gd4 128.74(10) . . ?
O18 Gd3 Gd4 35.15(8) . . ?
O20 Gd3 Gd4 73.64(9) . . ?
O3W Gd3 Gd4 157.40(11) . . ?
Gd2 Gd3 Gd4 58.861(10) . . ?
Gd1 Gd3 Gd4 58.669(9) . . ?
O1 Gd4 O19 131.03(14) 2_565 . ?
O1 Gd4 O13 85.37(17) 2_565 . ?
O19 Gd4 O13 135.64(14) . . ?
O1 Gd4 O15 83.16(16) 2_565 4_467 ?
O19 Gd4 O15 76.68(14) . 4_467 ?
O13 Gd4 O15 140.98(15) . 4_467 ?
O1 Gd4 O17 71.32(13) 2_565 . ?
O19 Gd4 O17 70.65(12) . . ?
O13 Gd4 O17 108.19(12) . . ?
O15 Gd4 O17 103.13(13) 4_467 . ?
O1 Gd4 O18 120.75(13) 2_565 . ?
O19 Gd4 O18 69.14(12) . . ?
O13 Gd4 O18 70.06(13) . . ?
O15 Gd4 O18 145.79(13) 4_467 . ?
O17 Gd4 O18 67.26(12) . . ?
O1 Gd4 O2 145.18(14) 2_565 3_656 ?
O19 Gd4 O2 74.24(13) . 3_656 ?
O13 Gd4 O2 88.09(15) . 3_656 ?
O15 Gd4 O2 80.67(15) 4_467 3_656 ?
O17 Gd4 O2 142.57(13) . 3_656 ?
O18 Gd4 O2 88.53(12) . 3_656 ?
O1 Gd4 O4W 71.40(14) 2_565 . ?
O19 Gd4 O4W 136.52(14) . . ?
O13 Gd4 O4W 71.55(13) . . ?
O15 Gd4 O4W 69.44(14) 4_467 . ?
O17 Gd4 O4W 142.60(13) . . ?
O18 Gd4 O4W 138.14(12) . . ?
O2 Gd4 O4W 74.08(14) 3_656 . ?
O1 Gd4 Gd2 148.18(10) 2_565 . ?
O19 Gd4 Gd2 37.81(9) . . ?
O13 Gd4 Gd2 97.84(11) . . ?
O15 Gd4 Gd2 111.25(11) 4_467 . ?
O17 Gd4 Gd2 77.68(8) . . ?
O18 Gd4 Gd2 35.87(8) . . ?
O2 Gd4 Gd2 66.61(10) 3_656 . ?
O4W Gd4 Gd2 139.67(9) . . ?
O1 Gd4 Gd1 96.16(11) 2_565 . ?
O19 Gd4 Gd1 36.01(9) . . ?
O13 Gd4 Gd1 141.80(9) . . ?
O15 Gd4 Gd1 76.65(11) 4_467 . ?
O17 Gd4 Gd1 39.13(8) . . ?
O18 Gd4 Gd1 76.69(8) . . ?
O2 Gd4 Gd1 109.67(10) 3_656 . ?
O4W Gd4 Gd1 144.88(9) . . ?
Gd2 Gd4 Gd1 62.175(14) . . ?
O1 Gd4 Gd3 90.79(10) 2_565 . ?
O19 Gd4 Gd3 74.06(9) . . ?
O13 Gd4 Gd3 82.40(9) . . ?
O15 Gd4 Gd3 134.78(11) 4_467 . ?
O17 Gd4 Gd3 34.24(8) . . ?
O18 Gd4 Gd3 34.86(8) . . ?
O2 Gd4 Gd3 122.16(9) 3_656 . ?
O4W Gd4 Gd3 149.19(10) . . ?
Gd2 Gd4 Gd3 58.624(9) . . ?
Gd1 Gd4 Gd3 59.447(10) . . ?
S1 O1 Gd4 158.3(3) . 2_564 ?
S1 O2 Gd4 130.0(2) . 3_646 ?
S1 O3 Gd2 158.6(3) . . ?
S1 O4 Gd2 128.8(2) 3_656 . ?
S2 O5 Gd3 169.4(3) . 2_564 ?
S2 O6 Gd2 117.0(2) . 3_656 ?
S2 O7 Gd2 153.7(3) . . ?
S2 O8 Gd3 142.7(3) 3_646 . ?
S3 O9 Gd3 150.7(2) . 2_564 ?
S3 O10 Gd1 166.4(3) . . ?
S3 O11 Gd1 137.5(2) 3_546 . ?
S3 O12 Gd3 128.7(3) 3_546 . ?
S4 O13 Gd4 154.6(2) . . ?
S4 O14 Gd1 160.3(3) . 2_565 ?
S4 O15 Gd4 122.7(2) . 4_567 ?
S4 O16 Gd1 138.5(2) 4_467 . ?
Gd3 O17 Gd4 110.93(13) . . ?
Gd3 O17 Gd1 105.14(13) . . ?
Gd4 O17 Gd1 102.88(13) . . ?
Gd2 O18 Gd3 106.85(13) . . ?
Gd2 O18 Gd4 106.67(14) . . ?
Gd3 O18 Gd4 109.99(13) . . ?
Gd4 O19 Gd1 108.30(15) . . ?
Gd4 O19 Gd2 105.78(14) . . ?
Gd1 O19 Gd2 110.57(14) . . ?
Gd1 O20 Gd2 111.70(15) . . ?
Gd1 O20 Gd3 107.82(14) . . ?
Gd2 O20 Gd3 103.79(14) . . ?
O1 S1 O3 108.4(3) . . ?
O1 S1 O2 109.6(3) . . ?
O3 S1 O2 109.9(3) . . ?
O1 S1 O4 110.1(2) . 3_646 ?
O3 S1 O4 109.3(3) . 3_646 ?
O2 S1 O4 109.5(2) . 3_646 ?
O5 S2 O7 109.7(3) . . ?
O5 S2 O8 110.4(3) . 3_656 ?
O7 S2 O8 108.0(3) . 3_656 ?
O5 S2 O6 111.1(3) . . ?
O7 S2 O6 110.6(3) . . ?
O8 S2 O6 107.0(3) 3_656 . ?
O10 S3 O9 109.5(3) . . ?
O10 S3 O11 109.6(2) . 3_556 ?
O9 S3 O11 108.3(2) . 3_556 ?
O10 S3 O12 110.3(3) . 3_556 ?
O9 S3 O12 111.1(3) . 3_556 ?
O11 S3 O12 108.1(2) 3_556 3_556 ?
O14 S4 O13 109.3(3) . . ?
O14 S4 O15 110.9(3) . . ?
O13 S4 O15 110.2(3) . . ?
O14 S4 O16 109.5(2) . 4_567 ?
O13 S4 O16 107.8(2) . 4_567 ?
O15 S4 O16 109.0(2) . 4_567 ?

_diffrn_measured_fraction_theta_max 0.993
_diffrn_reflns_theta_full        27.89
_diffrn_measured_fraction_theta_full 0.993
_refine_diff_density_max         1.342
_refine_diff_density_min         -1.059
_refine_diff_density_rms         0.241
_database_code_depnum_ccdc_archive 'CCDC 981569'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_1

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Dy4 H10 O23 S4'
_chemical_formula_sum            'Dy4 H10 O23 S4'
_chemical_formula_weight         1156.32

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           ?
_symmetry_space_group_name_H-M   ?

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y+1/2, -z'
'-x, y+1/2, -z+1/2'

_cell_length_a                   10.278(2)
_cell_length_b                   10.761(2)
_cell_length_c                   16.613(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     1837.4(6)
_cell_formula_units_Z            4
_cell_measurement_temperature    113(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.07
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.180
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2088
_exptl_absorpt_coefficient_mu    16.650
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.105
_exptl_absorpt_correction_T_max  0.312
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      113(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'Rotating Anode'
_diffrn_radiation_monochromator  Confocal
_diffrn_radiation_detector       CCD
_diffrn_measurement_device       
;
Saturn70 (4x4 bin mode)
;
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            14990
_diffrn_reflns_av_R_equivalents  0.1982
_diffrn_reflns_av_sigmaI/netI    0.1102
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_theta_min         2.25
_diffrn_reflns_theta_max         25.01
_reflns_number_total             3246
_reflns_number_gt                3182
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.1125P)²+150.9352P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0031(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.11(5)
_refine_ls_number_reflns         3246
_refine_ls_number_parameters     281
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0891
_refine_ls_R_factor_gt           0.0873
_refine_ls_wR_factor_ref         0.2028
_refine_ls_wR_factor_gt          0.2018
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_restrained_S_all      1.060
_refine_ls_shift/su_max          9.036
_refine_ls_shift/su_mean         0.145

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Dy1 Dy 0.74200(11) -0.19395(12) 0.55174(9) 0.0069(4) Uani 1 1 d . . .
Dy2 Dy 0.55622(13) 0.01885(13) 0.69452(8) 0.0066(4) Uani 1 1 d . . .
Dy3 Dy 0.92875(13) -0.02044(13) 0.71221(8) 0.0068(4) Uani 1 1 d . . .
Dy4 Dy 0.78178(12) 0.16105(12) 0.54278(9) 0.0085(4) Uani 1 1 d . . .
O1 O 1.008(3) 0.097(2) 0.3052(14) 0.026(6) Uani 1 1 d . . .
O2 O 1.002(3) 0.298(3) 0.3766(18) 0.041(7) Uani 1 1 d . . .
O3 O 1.1694(19) 0.153(2) 0.4082(13) 0.018(5) Uani 1 1 d . . .
O4 O 0.941(2) 0.118(2) 0.4457(12) 0.017(5) Uani 1 1 d . . .
O5 O 1.183(3) 0.259(3) 0.5676(16) 0.038(8) Uani 1 1 d . . .
O6 O 0.952(2) 0.292(2) 0.5850(18) 0.031(7) Uani 1 1 d . . .
O7 O 1.108(3) 0.339(3) 0.6891(14) 0.043(9) Uani 1 1 d . . .
O8 O 1.065(2) 0.130(2) 0.6557(16) 0.029(6) Uani 1 1 d . . .
O9 O 0.918(3) 0.334(2) 0.8355(15) 0.028(6) Uani 1 1 d . . .
O10 O 1.101(2) 0.203(2) 0.8674(13) 0.022(5) Uani 1 1 d . . .
O11 O 0.9083(19) 0.202(3) 0.9495(13) 0.025(6) Uani 1 1 d . . .
O12 O 0.901(2) 0.113(2) 0.8210(13) 0.022(6) Uani 1 1 d . . .
O13 O 0.5926(18) 0.157(2) 0.7990(12) 0.014(5) Uani 1 1 d . . .
O14 O 0.554(2) 0.352(2) 0.8625(16) 0.021(5) Uani 1 1 d . . .
O15 O 0.6336(19) 0.177(2) 0.9379(12) 0.020(6) Uani 1 1 d . . .
O16 O 0.409(2) 0.181(2) 0.8899(15) 0.024(6) Uani 1 1 d . . .
O17 O 0.727(2) -0.1205(19) 0.6877(13) 0.016(5) Uani 1 1 d . . .
H17 H 0.7137 -0.1895 0.7253 0.019 Uiso 1 1 d R . .
O18 O 0.6363(17) -0.0015(17) 0.5545(12) 0.006(4) Uani 1 1 d . . .
H18 H 0.5659 0.0038 0.5149 0.007 Uiso 1 1 d R . .
O19 O 0.8822(19) -0.025(2) 0.5750(13) 0.015(5) Uani 1 1 d . . .
H19 H 0.9626 -0.0349 0.5440 0.018 Uiso 1 1 d R . .
O20 O 0.765(2) 0.122(2) 0.6775(13) 0.017(5) Uani 1 1 d . . .
H20 H 0.7706 0.1985 0.7093 0.021 Uiso 1 1 d R . .
O1W O 0.764(2) -0.410(2) 0.5002(14) 0.023(5) Uani 1 1 d . . .
O2W O 0.333(3) 0.065(4) 0.7001(19) 0.048(9) Uani 1 1 d . . .
O3W O 1.136(2) -0.018(2) 0.7929(16) 0.024(6) Uani 1 1 d . . .
S1 S 1.0281(7) 0.1659(7) 0.3834(4) 0.0091(15) Uani 1 1 d . . .
S2 S 1.0746(7) 0.2525(7) 0.6240(4) 0.0106(15) Uani 1 1 d . . .
S3 S 0.9564(7) 0.2143(7) 0.8689(4) 0.0116(15) Uani 1 1 d . . .
S4 S 0.5461(7) 0.2152(8) 0.8727(4) 0.0111(15) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Dy1 O16 2.27(2) 4_646 ?
Dy1 O15 2.289(18) 2_654 ?
Dy1 O11 2.298(17) 2_654 ?
Dy1 O18 2.339(19) . ?
Dy1 O19 2.35(2) . ?
Dy1 O10 2.37(2) 4_746 ?
Dy1 O17 2.40(2) . ?
Dy1 O1W 2.49(2) . ?
Dy1 Dy3 3.7786(19) . ?
Dy1 Dy2 3.8101(19) . ?
Dy1 Dy4 3.845(2) . ?
Dy2 O17 2.31(2) . ?
Dy2 O13 2.313(19) . ?
Dy2 O1 2.318(19) 2_655 ?
Dy2 O14 2.33(2) 4_646 ?
Dy2 O2W 2.35(3) . ?
Dy2 O2 2.36(3) 3_456 ?
Dy2 O20 2.43(2) . ?
Dy2 O18 2.476(19) . ?
Dy2 Dy4 3.751(2) . ?
Dy2 Dy3 3.863(2) . ?
Dy3 O7 2.26(3) 4_746 ?
Dy3 O19 2.33(2) . ?
Dy3 O12 2.330(19) . ?
Dy3 O8 2.34(2) . ?
Dy3 O20 2.35(2) . ?
Dy3 O9 2.36(3) 4_746 ?
Dy3 O17 2.37(2) . ?
Dy3 O3W 2.52(2) . ?
Dy3 Dy4 3.744(2) . ?
Dy4 O5 2.27(2) 3_456 ?
Dy4 O20 2.28(2) . ?
Dy4 O18 2.309(17) . ?
Dy4 O19 2.32(2) . ?
Dy4 O4 2.35(2) . ?
Dy4 O6 2.35(3) . ?
Dy4 O3 2.45(2) 3_456 ?
O1 S1 1.51(2) . ?
O1 Dy2 2.318(19) 2_654 ?
O2 S1 1.45(3) . ?
O2 Dy2 2.36(3) 3_556 ?
O3 S1 1.52(2) . ?
O3 Dy4 2.45(2) 3_556 ?
O4 S1 1.46(2) . ?
O5 S2 1.46(2) . ?
O5 Dy4 2.27(2) 3_556 ?
O6 S2 1.48(2) . ?
O7 S2 1.47(2) . ?
O7 Dy3 2.26(2) 4_756 ?
O8 S2 1.42(3) . ?
O9 S3 1.45(3) . ?
O9 Dy3 2.36(3) 4_756 ?
O10 S3 1.49(2) . ?
O10 Dy1 2.37(2) 4_756 ?
O11 S3 1.43(2) . ?
O11 Dy1 2.298(17) 2_655 ?
O12 S3 1.46(2) . ?
O13 S4 1.46(2) . ?
O14 S4 1.48(2) . ?
O14 Dy2 2.33(2) 4_656 ?
O15 S4 1.468(19) . ?
O15 Dy1 2.289(18) 2_655 ?
O16 S4 1.48(3) . ?
O16 Dy1 2.27(2) 4_656 ?
O17 H17 0.9800 . ?
O18 H18 0.9800 . ?
O19 H19 0.9800 . ?
O20 H20 0.9800 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Dy1 O15 141.4(9) 4_646 2_654 ?
O16 Dy1 O11 80.4(9) 4_646 2_654 ?
O15 Dy1 O11 76.6(8) 2_654 2_654 ?
O16 Dy1 O18 101.5(8) 4_646 . ?
O15 Dy1 O18 101.8(8) 2_654 . ?
O11 Dy1 O18 74.7(8) 2_654 . ?
O16 Dy1 O19 143.7(8) 4_646 . ?
O15 Dy1 O19 74.4(8) 2_654 . ?
O11 Dy1 O19 124.3(9) 2_654 . ?
O18 Dy1 O19 66.2(7) . . ?
O16 Dy1 O10 86.9(8) 4_646 4_746 ?
O15 Dy1 O10 97.2(8) 2_654 4_746 ?
O11 Dy1 O10 149.0(9) 2_654 4_746 ?
O18 Dy1 O10 135.9(8) . 4_746 ?
O19 Dy1 O10 81.5(9) . 4_746 ?
O16 Dy1 O17 75.5(8) 4_646 . ?
O15 Dy1 O17 141.9(8) 2_654 . ?
O11 Dy1 O17 131.7(8) 2_654 . ?
O18 Dy1 O17 70.1(7) . . ?
O19 Dy1 O17 68.3(7) . . ?
O10 Dy1 O17 70.4(8) 4_746 . ?
O16 Dy1 O1W 69.8(9) 4_646 . ?
O15 Dy1 O1W 75.0(9) 2_654 . ?
O11 Dy1 O1W 76.8(9) 2_654 . ?
O18 Dy1 O1W 151.2(7) . . ?
O19 Dy1 O1W 136.3(8) . . ?
O10 Dy1 O1W 72.3(9) 4_746 . ?
O17 Dy1 O1W 129.7(7) . . ?
O16 Dy1 Dy3 109.8(6) 4_646 . ?
O15 Dy1 Dy3 105.0(6) 2_654 . ?
O11 Dy1 Dy3 151.9(7) 2_654 . ?
O18 Dy1 Dy3 77.5(5) . . ?
O19 Dy1 Dy3 36.0(5) . . ?
O10 Dy1 Dy3 59.2(7) 4_746 . ?
O17 Dy1 Dy3 37.4(5) . . ?
O1W Dy1 Dy3 131.2(6) . . ?
O16 Dy1 Dy2 75.4(7) 4_646 . ?
O15 Dy1 Dy2 138.2(6) 2_654 . ?
O11 Dy1 Dy2 98.4(6) 2_654 . ?
O18 Dy1 Dy2 39.0(5) . . ?
O19 Dy1 Dy2 74.9(5) . . ?
O10 Dy1 Dy2 105.6(6) 4_746 . ?
O17 Dy1 Dy2 35.2(5) . . ?
O1W Dy1 Dy2 145.2(6) . . ?
Dy3 Dy1 Dy2 61.21(4) . . ?
O16 Dy1 Dy4 132.7(7) 4_646 . ?
O15 Dy1 Dy4 80.1(6) 2_654 . ?
O11 Dy1 Dy4 94.6(7) 2_654 . ?
O18 Dy1 Dy4 33.9(4) . . ?
O19 Dy1 Dy4 34.2(6) . . ?
O10 Dy1 Dy4 114.5(7) 4_746 . ?
O17 Dy1 Dy4 73.5(5) . . ?
O1W Dy1 Dy4 154.9(6) . . ?
Dy3 Dy1 Dy4 58.82(3) . . ?
Dy2 Dy1 Dy4 58.68(4) . . ?
O17 Dy2 O13 109.3(7) . . ?
O17 Dy2 O1 84.5(9) . 2_655 ?
O13 Dy2 O1 78.2(9) . 2_655 ?
O17 Dy2 O14 81.3(8) . 4_646 ?
O13 Dy2 O14 151.6(8) . 4_646 ?
O1 Dy2 O14 76.6(10) 2_655 4_646 ?
O17 Dy2 O2W 151.7(11) . . ?
O13 Dy2 O2W 89.6(10) . . ?
O1 Dy2 O2W 78.9(10) 2_655 . ?
O14 Dy2 O2W 72.8(11) 4_646 . ?
O17 Dy2 O2 134.1(9) . 3_456 ?
O13 Dy2 O2 83.1(9) . 3_456 ?
O1 Dy2 O2 141.1(10) 2_655 3_456 ?
O14 Dy2 O2 109.0(9) 4_646 3_456 ?
O2W Dy2 O2 67.2(11) . 3_456 ?
O17 Dy2 O20 67.7(8) . . ?
O13 Dy2 O20 69.7(7) . . ?
O1 Dy2 O20 126.0(8) 2_655 . ?
O14 Dy2 O20 137.2(9) 4_646 . ?
O2W Dy2 O20 140.3(11) . . ?
O2 Dy2 O20 76.7(9) 3_456 . ?
O17 Dy2 O18 69.2(7) . . ?
O13 Dy2 O18 135.0(7) . . ?
O1 Dy2 O18 142.3(8) 2_655 . ?
O14 Dy2 O18 73.2(8) 4_646 . ?
O2W Dy2 O18 112.3(9) . . ?
O2 Dy2 O18 71.5(9) 3_456 . ?
O20 Dy2 O18 68.8(7) . . ?
O17 Dy2 Dy4 76.3(6) . . ?
O13 Dy2 Dy4 98.2(5) . . ?
O1 Dy2 Dy4 158.1(6) 2_655 . ?
O14 Dy2 Dy4 110.0(7) 4_646 . ?
O2W Dy2 Dy4 122.9(8) . . ?
O2 Dy2 Dy4 58.0(8) 3_456 . ?
O20 Dy2 Dy4 35.9(5) . . ?
O18 Dy2 Dy4 36.8(4) . . ?
O17 Dy2 Dy1 36.8(5) . . ?
O13 Dy2 Dy1 140.5(5) . . ?
O1 Dy2 Dy1 108.1(7) 2_655 . ?
O14 Dy2 Dy1 61.7(6) 4_646 . ?
O2W Dy2 Dy1 129.9(9) . . ?
O2 Dy2 Dy1 108.0(7) 3_456 . ?
O20 Dy2 Dy1 76.1(6) . . ?
O18 Dy2 Dy1 36.5(4) . . ?
Dy4 Dy2 Dy1 61.12(4) . . ?
O17 Dy2 Dy3 34.9(5) . . ?
O13 Dy2 Dy3 81.5(5) . . ?
O1 Dy2 Dy3 99.3(6) 2_655 . ?
O14 Dy2 Dy3 115.4(6) 4_646 . ?
O2W Dy2 Dy3 171.1(9) . . ?
O2 Dy2 Dy3 111.3(7) 3_456 . ?
O20 Dy2 Dy3 35.3(5) . . ?
O18 Dy2 Dy3 74.5(4) . . ?
Dy4 Dy2 Dy3 58.88(3) . . ?
Dy1 Dy2 Dy3 58.99(3) . . ?
O7 Dy3 O19 131.4(9) 4_746 . ?
O7 Dy3 O12 80.1(10) 4_746 . ?
O19 Dy3 O12 138.3(8) . . ?
O7 Dy3 O8 148.8(10) 4_746 . ?
O19 Dy3 O8 75.2(8) . . ?
O12 Dy3 O8 87.6(10) . . ?
O7 Dy3 O20 119.6(11) 4_746 . ?
O19 Dy3 O20 68.1(8) . . ?
O12 Dy3 O20 72.4(8) . . ?
O8 Dy3 O20 82.9(9) . . ?
O7 Dy3 O9 84.9(11) 4_746 4_746 ?
O19 Dy3 O9 78.1(8) . 4_746 ?
O12 Dy3 O9 139.0(8) . 4_746 ?
O8 Dy3 O9 85.8(9) . 4_746 ?
O20 Dy3 O9 146.1(8) . 4_746 ?
O7 Dy3 O17 71.0(9) 4_746 . ?
O19 Dy3 O17 69.1(7) . . ?
O12 Dy3 O17 107.8(8) . . ?
O8 Dy3 O17 140.2(9) . . ?
O20 Dy3 O17 68.2(8) . . ?
O9 Dy3 O17 102.9(9) 4_746 . ?
O7 Dy3 O3W 76.4(9) 4_746 . ?
O19 Dy3 O3W 134.0(8) . . ?
O12 Dy3 O3W 71.6(8) . . ?
O8 Dy3 O3W 72.5(8) . . ?
O20 Dy3 O3W 136.8(8) . . ?
O9 Dy3 O3W 67.8(8) 4_746 . ?
O17 Dy3 O3W 146.9(7) . . ?
O7 Dy3 Dy4 145.6(8) 4_746 . ?
O19 Dy3 Dy4 36.2(6) . . ?
O12 Dy3 Dy4 102.2(6) . . ?
O8 Dy3 Dy4 65.0(7) . . ?
O20 Dy3 Dy4 35.5(6) . . ?
O9 Dy3 Dy4 111.3(6) 4_746 . ?
O17 Dy3 Dy4 75.8(5) . . ?
O3W Dy3 Dy4 137.3(5) . . ?
O7 Dy3 Dy1 95.5(7) 4_746 . ?
O19 Dy3 Dy1 36.4(5) . . ?
O12 Dy3 Dy1 142.2(5) . . ?
O8 Dy3 Dy1 111.3(7) . . ?
O20 Dy3 Dy1 77.6(5) . . ?
O9 Dy3 Dy1 76.9(6) 4_746 . ?
O17 Dy3 Dy1 37.8(5) . . ?
O3W Dy3 Dy1 144.2(6) . . ?
Dy4 Dy3 Dy1 61.47(4) . . ?
O7 Dy3 Dy2 87.7(9) 4_746 . ?
O19 Dy3 Dy2 74.0(5) . . ?
O12 Dy3 Dy2 82.4(5) . . ?
O8 Dy3 Dy2 119.1(7) . . ?
O20 Dy3 Dy2 36.9(6) . . ?
O9 Dy3 Dy2 135.0(6) 4_746 . ?
O17 Dy3 Dy2 33.9(5) . . ?
O3W Dy3 Dy2 151.4(6) . . ?
Dy4 Dy3 Dy2 59.06(3) . . ?
Dy1 Dy3 Dy2 59.80(3) . . ?
O5 Dy4 O20 146.1(10) 3_456 . ?
O5 Dy4 O18 93.8(9) 3_456 . ?
O20 Dy4 O18 74.3(7) . . ?
O5 Dy4 O19 135.7(10) 3_456 . ?
O20 Dy4 O19 69.3(8) . . ?
O18 Dy4 O19 67.3(7) . . ?
O5 Dy4 O4 80.4(9) 3_456 . ?
O20 Dy4 O4 133.5(8) . . ?
O18 Dy4 O4 111.1(7) . . ?
O19 Dy4 O4 71.0(7) . . ?
O5 Dy4 O6 110.3(11) 3_456 . ?
O20 Dy4 O6 82.7(10) . . ?
O18 Dy4 O6 155.4(8) . . ?
O19 Dy4 O6 96.7(7) . . ?
O4 Dy4 O6 78.7(9) . . ?
O5 Dy4 O3 75.3(10) 3_456 3_456 ?
O20 Dy4 O3 77.9(8) . 3_456 ?
O18 Dy4 O3 106.6(7) . 3_456 ?
O19 Dy4 O3 147.1(7) . 3_456 ?
O4 Dy4 O3 136.1(7) . 3_456 ?
O6 Dy4 O3 76.2(8) . 3_456 ?
O5 Dy4 Dy3 170.9(8) 3_456 . ?
O20 Dy4 Dy3 36.6(6) . . ?
O18 Dy4 Dy3 78.6(5) . . ?
O19 Dy4 Dy3 36.4(5) . . ?
O4 Dy4 Dy3 97.5(6) . . ?
O6 Dy4 Dy3 77.8(6) . . ?
O3 Dy4 Dy3 111.5(5) 3_456 . ?
O5 Dy4 Dy2 115.0(7) 3_456 . ?
O20 Dy4 Dy2 38.8(6) . . ?
O18 Dy4 Dy2 40.0(5) . . ?
O19 Dy4 Dy2 76.5(5) . . ?
O4 Dy4 Dy2 144.3(5) . . ?
O6 Dy4 Dy2 120.2(8) . . ?
O3 Dy4 Dy2 79.6(6) 3_456 . ?
Dy3 Dy4 Dy2 62.05(4) . . ?
O5 Dy4 Dy1 111.2(8) 3_456 . ?
O20 Dy4 Dy1 76.8(6) . . ?
O18 Dy4 Dy1 34.4(5) . . ?
O19 Dy4 Dy1 34.8(5) . . ?
O4 Dy4 Dy1 84.4(5) . . ?
O6 Dy4 Dy1 131.5(6) . . ?
O3 Dy4 Dy1 138.5(6) 3_456 . ?
Dy3 Dy4 Dy1 59.70(4) . . ?
Dy2 Dy4 Dy1 60.19(3) . . ?
S1 O1 Dy2 170.5(17) . 2_654 ?
S1 O2 Dy2 144.2(17) . 3_556 ?
S1 O3 Dy4 117.6(14) . 3_556 ?
S1 O4 Dy4 147.3(14) . . ?
S2 O5 Dy4 151.7(19) . 3_556 ?
S2 O6 Dy4 126.4(15) . . ?
S2 O7 Dy3 157(2) . 4_756 ?
S2 O8 Dy3 146.5(17) . . ?
S3 O9 Dy3 122.5(16) . 4_756 ?
S3 O10 Dy1 128.9(13) . 4_756 ?
S3 O11 Dy1 157.8(15) . 2_655 ?
S3 O12 Dy3 146.2(15) . . ?
S4 O13 Dy2 148.7(12) . . ?
S4 O14 Dy2 141.9(14) . 4_656 ?
S4 O15 Dy1 158.3(16) . 2_655 ?
S4 O16 Dy1 125.7(14) . 4_656 ?
Dy2 O17 Dy3 111.1(8) . . ?
Dy2 O17 Dy1 108.0(8) . . ?
Dy3 O17 Dy1 104.8(9) . . ?
Dy2 O17 H17 110.7 . . ?
Dy3 O17 H17 110.9 . . ?
Dy1 O17 H17 111.1 . . ?
Dy4 O18 Dy1 111.6(7) . . ?
Dy4 O18 Dy2 103.2(7) . . ?
Dy1 O18 Dy2 104.6(7) . . ?
Dy4 O18 H18 112.2 . . ?
Dy1 O18 H18 112.4 . . ?
Dy2 O18 H18 112.3 . . ?
Dy4 O19 Dy3 107.4(8) . . ?
Dy4 O19 Dy1 110.9(8) . . ?
Dy3 O19 Dy1 107.7(8) . . ?
Dy4 O19 H19 110.3 . . ?
Dy3 O19 H19 110.2 . . ?
Dy1 O19 H19 110.3 . . ?
Dy4 O20 Dy3 107.9(10) . . ?
Dy4 O20 Dy2 105.3(8) . . ?
Dy3 O20 Dy2 107.8(9) . . ?
Dy4 O20 H20 111.8 . . ?
Dy3 O20 H20 112.0 . . ?
Dy2 O20 H20 111.7 . . ?
O2 S1 O4 106.9(15) . . ?
O2 S1 O1 112.7(17) . . ?
O4 S1 O1 110.5(14) . . ?
O2 S1 O3 107.0(16) . . ?
O4 S1 O3 111.0(13) . . ?
O1 S1 O3 108.8(14) . . ?
O8 S2 O5 109.6(17) . . ?
O8 S2 O7 109.5(17) . . ?
O5 S2 O7 105.2(19) . . ?
O8 S2 O6 111.4(15) . . ?
O5 S2 O6 110.9(17) . . ?
O7 S2 O6 110.0(16) . . ?
O11 S3 O9 110.2(16) . . ?
O11 S3 O12 107.7(16) . . ?
O9 S3 O12 110.0(14) . . ?
O11 S3 O10 110.5(13) . . ?
O9 S3 O10 109.7(16) . . ?
O12 S3 O10 108.7(13) . . ?
O13 S4 O15 107.3(13) . . ?
O13 S4 O16 111.4(12) . . ?
O15 S4 O16 111.7(14) . . ?
O13 S4 O14 108.4(15) . . ?
O15 S4 O14 109.3(15) . . ?
O16 S4 O14 108.7(14) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O16 Dy1 Dy2 O17 85.4(11) 4_646 . . . ?
O15 Dy1 Dy2 O17 -117.6(12) 2_654 . . . ?
O11 Dy1 Dy2 O17 163.1(11) 2_654 . . . ?
O18 Dy1 Dy2 O17 -144.2(11) . . . . ?
O19 Dy1 Dy2 O17 -73.5(11) . . . . ?
O10 Dy1 Dy2 O17 3.0(11) 4_746 . . . ?
O1W Dy1 Dy2 O17 84.3(14) . . . . ?
Dy3 Dy1 Dy2 O17 -37.5(9) . . . . ?
Dy4 Dy1 Dy2 O17 -106.5(9) . . . . ?
O16 Dy1 Dy2 O13 126.2(11) 4_646 . . . ?
O15 Dy1 Dy2 O13 -76.8(12) 2_654 . . . ?
O11 Dy1 Dy2 O13 -156.0(12) 2_654 . . . ?
O18 Dy1 Dy2 O13 -103.3(12) . . . . ?
O19 Dy1 Dy2 O13 -32.7(11) . . . . ?
O10 Dy1 Dy2 O13 43.8(11) 4_746 . . . ?
O17 Dy1 Dy2 O13 40.8(13) . . . . ?
O1W Dy1 Dy2 O13 125.1(14) . . . . ?
Dy3 Dy1 Dy2 O13 3.4(9) . . . . ?
Dy4 Dy1 Dy2 O13 -65.7(9) . . . . ?
O16 Dy1 Dy2 O1 32.8(9) 4_646 . . 2_655 ?
O15 Dy1 Dy2 O1 -170.2(11) 2_654 . . 2_655 ?
O11 Dy1 Dy2 O1 110.6(10) 2_654 . . 2_655 ?
O18 Dy1 Dy2 O1 163.2(10) . . . 2_655 ?
O19 Dy1 Dy2 O1 -126.1(9) . . . 2_655 ?
O10 Dy1 Dy2 O1 -49.6(10) 4_746 . . 2_655 ?
O17 Dy1 Dy2 O1 -52.6(11) . . . 2_655 ?
O1W Dy1 Dy2 O1 31.7(13) . . . 2_655 ?
Dy3 Dy1 Dy2 O1 -90.0(7) . . . 2_655 ?
Dy4 Dy1 Dy2 O1 -159.1(7) . . . 2_655 ?
O16 Dy1 Dy2 O14 -30.2(9) 4_646 . . 4_646 ?
O15 Dy1 Dy2 O14 126.7(10) 2_654 . . 4_646 ?
O11 Dy1 Dy2 O14 47.5(9) 2_654 . . 4_646 ?
O18 Dy1 Dy2 O14 100.2(10) . . . 4_646 ?
O19 Dy1 Dy2 O14 170.8(9) . . . 4_646 ?
O10 Dy1 Dy2 O14 -112.7(9) 4_746 . . 4_646 ?
O17 Dy1 Dy2 O14 -115.6(11) . . . 4_646 ?
O1W Dy1 Dy2 O14 -31.4(12) . . . 4_646 ?
Dy3 Dy1 Dy2 O14 -153.1(7) . . . 4_646 ?
Dy4 Dy1 Dy2 O14 137.8(7) . . . 4_646 ?
O16 Dy1 Dy2 O2W -57.7(12) 4_646 . . . ?
O15 Dy1 Dy2 O2W 99.3(14) 2_654 . . . ?
O11 Dy1 Dy2 O2W 20.1(12) 2_654 . . . ?
O18 Dy1 Dy2 O2W 72.7(13) . . . . ?
O19 Dy1 Dy2 O2W 143.4(12) . . . . ?
O10 Dy1 Dy2 O2W -140.1(13) 4_746 . . . ?
O17 Dy1 Dy2 O2W -143.1(14) . . . . ?
O1W Dy1 Dy2 O2W -58.8(15) . . . . ?
Dy3 Dy1 Dy2 O2W 179.5(11) . . . . ?
Dy4 Dy1 Dy2 O2W 110.4(11) . . . . ?
O16 Dy1 Dy2 O2 -132.6(9) 4_646 . . 3_456 ?
O15 Dy1 Dy2 O2 24.4(11) 2_654 . . 3_456 ?
O11 Dy1 Dy2 O2 -54.9(10) 2_654 . . 3_456 ?
O18 Dy1 Dy2 O2 -2.2(10) . . . 3_456 ?
O19 Dy1 Dy2 O2 68.5(9) . . . 3_456 ?
O10 Dy1 Dy2 O2 145.0(10) 4_746 . . 3_456 ?
O17 Dy1 Dy2 O2 142.0(11) . . . 3_456 ?
O1W Dy1 Dy2 O2 -133.7(12) . . . 3_456 ?
Dy3 Dy1 Dy2 O2 104.5(7) . . . 3_456 ?
Dy4 Dy1 Dy2 O2 35.5(7) . . . 3_456 ?
O16 Dy1 Dy2 O20 156.6(8) 4_646 . . . ?
O15 Dy1 Dy2 O20 -46.4(10) 2_654 . . . ?
O11 Dy1 Dy2 O20 -125.7(8) 2_654 . . . ?
O18 Dy1 Dy2 O20 -73.0(8) . . . . ?
O19 Dy1 Dy2 O20 -2.3(8) . . . . ?
O10 Dy1 Dy2 O20 74.2(8) 4_746 . . . ?
O17 Dy1 Dy2 O20 71.2(10) . . . . ?
O1W Dy1 Dy2 O20 155.5(11) . . . . ?
Dy3 Dy1 Dy2 O20 33.7(5) . . . . ?
Dy4 Dy1 Dy2 O20 -35.3(5) . . . . ?
O16 Dy1 Dy2 O18 -130.4(9) 4_646 . . . ?
O15 Dy1 Dy2 O18 26.6(11) 2_654 . . . ?
O11 Dy1 Dy2 O18 -52.7(9) 2_654 . . . ?
O19 Dy1 Dy2 O18 70.7(9) . . . . ?
O10 Dy1 Dy2 O18 147.2(9) 4_746 . . . ?
O17 Dy1 Dy2 O18 144.2(11) . . . . ?
O1W Dy1 Dy2 O18 -131.5(12) . . . . ?
Dy3 Dy1 Dy2 O18 106.7(7) . . . . ?
Dy4 Dy1 Dy2 O18 37.6(7) . . . . ?
O16 Dy1 Dy2 Dy4 -168.0(6) 4_646 . . . ?
O15 Dy1 Dy2 Dy4 -11.1(8) 2_654 . . . ?
O11 Dy1 Dy2 Dy4 -90.3(7) 2_654 . . . ?
O18 Dy1 Dy2 Dy4 -37.6(7) . . . . ?
O19 Dy1 Dy2 Dy4 33.0(6) . . . . ?
O10 Dy1 Dy2 Dy4 109.5(6) 4_746 . . . ?
O17 Dy1 Dy2 Dy4 106.5(9) . . . . ?
O1W Dy1 Dy2 Dy4 -169.2(10) . . . . ?
Dy3 Dy1 Dy2 Dy4 69.08(4) . . . . ?
O16 Dy1 Dy2 Dy3 122.9(6) 4_646 . . . ?
O15 Dy1 Dy2 Dy3 -80.2(8) 2_654 . . . ?
O11 Dy1 Dy2 Dy3 -159.4(7) 2_654 . . . ?
O18 Dy1 Dy2 Dy3 -106.7(7) . . . . ?
O19 Dy1 Dy2 Dy3 -36.0(6) . . . . ?
O10 Dy1 Dy2 Dy3 40.4(6) 4_746 . . . ?
O17 Dy1 Dy2 Dy3 37.5(9) . . . . ?
O1W Dy1 Dy2 Dy3 121.7(10) . . . . ?
Dy4 Dy1 Dy2 Dy3 -69.08(4) . . . . ?
O16 Dy1 Dy3 O7 24.4(12) 4_646 . . 4_746 ?
O15 Dy1 Dy3 O7 -138.7(11) 2_654 . . 4_746 ?
O11 Dy1 Dy3 O7 131.7(16) 2_654 . . 4_746 ?
O18 Dy1 Dy3 O7 122.3(10) . . . 4_746 ?
O19 Dy1 Dy3 O7 -171.2(13) . . . 4_746 ?
O10 Dy1 Dy3 O7 -49.2(11) 4_746 . . 4_746 ?
O17 Dy1 Dy3 O7 48.8(13) . . . 4_746 ?
O1W Dy1 Dy3 O7 -55.7(12) . . . 4_746 ?
Dy2 Dy1 Dy3 O7 84.2(9) . . . 4_746 ?
Dy4 Dy1 Dy3 O7 153.0(9) . . . 4_746 ?
O16 Dy1 Dy3 O19 -164.4(11) 4_646 . . . ?
O15 Dy1 Dy3 O19 32.5(11) 2_654 . . . ?
O11 Dy1 Dy3 O19 -57.1(16) 2_654 . . . ?
O18 Dy1 Dy3 O19 -66.5(10) . . . . ?
O10 Dy1 Dy3 O19 122.0(11) 4_746 . . . ?
O17 Dy1 Dy3 O19 -140.0(12) . . . . ?
O1W Dy1 Dy3 O19 115.5(12) . . . . ?
Dy2 Dy1 Dy3 O19 -104.6(9) . . . . ?
Dy4 Dy1 Dy3 O19 -35.8(9) . . . . ?
O16 Dy1 Dy3 O12 -56.6(13) 4_646 . . . ?
O15 Dy1 Dy3 O12 140.3(13) 2_654 . . . ?
O11 Dy1 Dy3 O12 50.7(17) 2_654 . . . ?
O18 Dy1 Dy3 O12 41.3(12) . . . . ?
O19 Dy1 Dy3 O12 107.8(15) . . . . ?
O10 Dy1 Dy3 O12 -130.2(13) 4_746 . . . ?
O17 Dy1 Dy3 O12 -32.2(14) . . . . ?
O1W Dy1 Dy3 O12 -136.7(14) . . . . ?
Dy2 Dy1 Dy3 O12 3.2(11) . . . . ?
Dy4 Dy1 Dy3 O12 72.0(11) . . . . ?
O16 Dy1 Dy3 O8 -172.0(10) 4_646 . . . ?
O15 Dy1 Dy3 O8 25.0(10) 2_654 . . . ?
O11 Dy1 Dy3 O8 -64.6(15) 2_654 . . . ?
O18 Dy1 Dy3 O8 -74.1(8) . . . . ?
O19 Dy1 Dy3 O8 -7.6(11) . . . . ?
O10 Dy1 Dy3 O8 114.5(9) 4_746 . . . ?
O17 Dy1 Dy3 O8 -147.5(11) . . . . ?
O1W Dy1 Dy3 O8 107.9(10) . . . . ?
Dy2 Dy1 Dy3 O8 -112.2(7) . . . . ?
Dy4 Dy1 Dy3 O8 -43.3(7) . . . . ?
O16 Dy1 Dy3 O20 -94.7(10) 4_646 . . . ?
O15 Dy1 Dy3 O20 102.2(9) 2_654 . . . ?
O11 Dy1 Dy3 O20 12.6(14) 2_654 . . . ?
O18 Dy1 Dy3 O20 3.2(7) . . . . ?
O19 Dy1 Dy3 O20 69.7(11) . . . . ?
O10 Dy1 Dy3 O20 -168.3(9) 4_746 . . . ?
O17 Dy1 Dy3 O20 -70.3(10) . . . . ?
O1W Dy1 Dy3 O20 -174.8(10) . . . . ?
Dy2 Dy1 Dy3 O20 -34.9(6) . . . . ?
Dy4 Dy1 Dy3 O20 33.9(6) . . . . ?
O16 Dy1 Dy3 O9 107.9(10) 4_646 . . 4_746 ?
O15 Dy1 Dy3 O9 -55.2(10) 2_654 . . 4_746 ?
O11 Dy1 Dy3 O9 -144.8(15) 2_654 . . 4_746 ?
O18 Dy1 Dy3 O9 -154.3(8) . . . 4_746 ?
O19 Dy1 Dy3 O9 -87.7(12) . . . 4_746 ?
O10 Dy1 Dy3 O9 34.3(9) 4_746 . . 4_746 ?
O17 Dy1 Dy3 O9 132.3(11) . . . 4_746 ?
O1W Dy1 Dy3 O9 27.7(11) . . . 4_746 ?
Dy2 Dy1 Dy3 O9 167.6(7) . . . 4_746 ?
Dy4 Dy1 Dy3 O9 -123.5(7) . . . 4_746 ?
O16 Dy1 Dy3 O17 -24.4(11) 4_646 . . . ?
O15 Dy1 Dy3 O17 172.5(10) 2_654 . . . ?
O11 Dy1 Dy3 O17 82.9(15) 2_654 . . . ?
O18 Dy1 Dy3 O17 73.4(9) . . . . ?
O19 Dy1 Dy3 O17 140.0(12) . . . . ?
O10 Dy1 Dy3 O17 -98.0(10) 4_746 . . . ?
O1W Dy1 Dy3 O17 -104.5(11) . . . . ?
Dy2 Dy1 Dy3 O17 35.3(8) . . . . ?
Dy4 Dy1 Dy3 O17 104.2(8) . . . . ?
O16 Dy1 Dy3 O3W 98.8(12) 4_646 . . . ?
O15 Dy1 Dy3 O3W -64.3(11) 2_654 . . . ?
O11 Dy1 Dy3 O3W -153.9(15) 2_654 . . . ?
O18 Dy1 Dy3 O3W -163.3(10) . . . . ?
O19 Dy1 Dy3 O3W -96.8(13) . . . . ?
O10 Dy1 Dy3 O3W 25.2(11) 4_746 . . . ?
O17 Dy1 Dy3 O3W 123.2(12) . . . . ?
O1W Dy1 Dy3 O3W 18.7(12) . . . . ?
Dy2 Dy1 Dy3 O3W 158.6(9) . . . . ?
Dy4 Dy1 Dy3 O3W -132.6(9) . . . . ?
O16 Dy1 Dy3 Dy4 -128.6(7) 4_646 . . . ?
O15 Dy1 Dy3 Dy4 68.3(6) 2_654 . . . ?
O11 Dy1 Dy3 Dy4 -21.3(13) 2_654 . . . ?
O18 Dy1 Dy3 Dy4 -30.8(4) . . . . ?
O19 Dy1 Dy3 Dy4 35.8(9) . . . . ?
O10 Dy1 Dy3 Dy4 157.8(6) 4_746 . . . ?
O17 Dy1 Dy3 Dy4 -104.2(8) . . . . ?
O1W Dy1 Dy3 Dy4 151.3(8) . . . . ?
Dy2 Dy1 Dy3 Dy4 -68.86(4) . . . . ?
O16 Dy1 Dy3 Dy2 -59.8(7) 4_646 . . . ?
O15 Dy1 Dy3 Dy2 137.1(6) 2_654 . . . ?
O11 Dy1 Dy3 Dy2 47.6(13) 2_654 . . . ?
O18 Dy1 Dy3 Dy2 38.1(4) . . . . ?
O19 Dy1 Dy3 Dy2 104.6(9) . . . . ?
O10 Dy1 Dy3 Dy2 -133.3(6) 4_746 . . . ?
O17 Dy1 Dy3 Dy2 -35.3(8) . . . . ?
O1W Dy1 Dy3 Dy2 -139.9(8) . . . . ?
Dy4 Dy1 Dy3 Dy2 68.86(4) . . . . ?
O17 Dy2 Dy3 O7 -58.2(12) . . . 4_746 ?
O13 Dy2 Dy3 O7 84.5(10) . . . 4_746 ?
O1 Dy2 Dy3 O7 8.0(10) 2_655 . . 4_746 ?
O14 Dy2 Dy3 O7 -71.6(10) 4_646 . . 4_746 ?
O2W Dy2 Dy3 O7 85(5) . . . 4_746 ?
O2 Dy2 Dy3 O7 163.5(11) 3_456 . . 4_746 ?
O20 Dy2 Dy3 O7 151.0(12) . . . 4_746 ?
O18 Dy2 Dy3 O7 -133.9(9) . . . 4_746 ?
Dy4 Dy2 Dy3 O7 -170.5(8) . . . 4_746 ?
Dy1 Dy2 Dy3 O7 -97.7(8) . . . 4_746 ?
O17 Dy2 Dy3 O19 76.1(11) . . . . ?
O13 Dy2 Dy3 O19 -141.2(8) . . . . ?
O1 Dy2 Dy3 O19 142.3(9) 2_655 . . . ?
O14 Dy2 Dy3 O19 62.8(9) 4_646 . . . ?
O2W Dy2 Dy3 O19 -141(5) . . . . ?
O2 Dy2 Dy3 O19 -62.1(9) 3_456 . . . ?
O20 Dy2 Dy3 O19 -74.6(11) . . . . ?
O18 Dy2 Dy3 O19 0.4(8) . . . . ?
Dy4 Dy2 Dy3 O19 -36.2(6) . . . . ?
Dy1 Dy2 Dy3 O19 36.6(6) . . . . ?
O17 Dy2 Dy3 O12 -138.6(12) . . . . ?
O13 Dy2 Dy3 O12 4.1(9) . . . . ?
O1 Dy2 Dy3 O12 -72.4(10) 2_655 . . . ?
O14 Dy2 Dy3 O12 -151.9(10) 4_646 . . . ?
O2W Dy2 Dy3 O12 5(5) . . . . ?
O2 Dy2 Dy3 O12 83.2(11) 3_456 . . . ?
O20 Dy2 Dy3 O12 70.7(12) . . . . ?
O18 Dy2 Dy3 O12 145.7(8) . . . . ?
Dy4 Dy2 Dy3 O12 109.1(7) . . . . ?
Dy1 Dy2 Dy3 O12 -178.0(7) . . . . ?
O17 Dy2 Dy3 O8 138.5(13) . . . . ?
O13 Dy2 Dy3 O8 -78.9(10) . . . . ?
O1 Dy2 Dy3 O8 -155.4(10) 2_655 . . . ?
O14 Dy2 Dy3 O8 125.1(11) 4_646 . . . ?
O2W Dy2 Dy3 O8 -78(5) . . . . ?
O2 Dy2 Dy3 O8 0.2(11) 3_456 . . . ?
O20 Dy2 Dy3 O8 -12.3(12) . . . . ?
O18 Dy2 Dy3 O8 62.8(9) . . . . ?
Dy4 Dy2 Dy3 O8 26.2(8) . . . . ?
Dy1 Dy2 Dy3 O8 99.0(8) . . . . ?
O17 Dy2 Dy3 O20 150.7(13) . . . . ?
O13 Dy2 Dy3 O20 -66.6(11) . . . . ?
O1 Dy2 Dy3 O20 -143.1(11) 2_655 . . . ?
O14 Dy2 Dy3 O20 137.4(12) 4_646 . . . ?
O2W Dy2 Dy3 O20 -66(5) . . . . ?
O2 Dy2 Dy3 O20 12.5(12) 3_456 . . . ?
O18 Dy2 Dy3 O20 75.0(10) . . . . ?
Dy4 Dy2 Dy3 O20 38.4(9) . . . . ?
Dy1 Dy2 Dy3 O20 111.2(9) . . . . ?
O17 Dy2 Dy3 O9 22.3(14) . . . 4_746 ?
O13 Dy2 Dy3 O9 165.0(11) . . . 4_746 ?
O1 Dy2 Dy3 O9 88.5(12) 2_655 . . 4_746 ?
O14 Dy2 Dy3 O9 9.0(12) 4_646 . . 4_746 ?
O2W Dy2 Dy3 O9 165(5) . . . 4_746 ?
O2 Dy2 Dy3 O9 -115.9(12) 3_456 . . 4_746 ?
O20 Dy2 Dy3 O9 -128.4(13) . . . 4_746 ?
O18 Dy2 Dy3 O9 -53.4(10) . . . 4_746 ?
Dy4 Dy2 Dy3 O9 -90.0(9) . . . 4_746 ?
Dy1 Dy2 Dy3 O9 -17.2(9) . . . 4_746 ?
O13 Dy2 Dy3 O17 142.7(11) . . . . ?
O1 Dy2 Dy3 O17 66.2(12) 2_655 . . . ?
O14 Dy2 Dy3 O17 -13.3(12) 4_646 . . . ?
O2W Dy2 Dy3 O17 143(5) . . . . ?
O2 Dy2 Dy3 O17 -138.2(12) 3_456 . . . ?
O20 Dy2 Dy3 O17 -150.7(13) . . . . ?
O18 Dy2 Dy3 O17 -75.7(10) . . . . ?
Dy4 Dy2 Dy3 O17 -112.3(10) . . . . ?
Dy1 Dy2 Dy3 O17 -39.5(9) . . . . ?
O17 Dy2 Dy3 O3W -114.0(14) . . . . ?
O13 Dy2 Dy3 O3W 28.7(12) . . . . ?
O1 Dy2 Dy3 O3W -47.8(13) 2_655 . . . ?
O14 Dy2 Dy3 O3W -127.3(13) 4_646 . . . ?
O2W Dy2 Dy3 O3W 29(5) . . . . ?
O2 Dy2 Dy3 O3W 107.8(13) 3_456 . . . ?
O20 Dy2 Dy3 O3W 95.3(14) . . . . ?
O18 Dy2 Dy3 O3W 170.3(11) . . . . ?
Dy4 Dy2 Dy3 O3W 133.7(10) . . . . ?
Dy1 Dy2 Dy3 O3W -153.5(10) . . . . ?
O17 Dy2 Dy3 Dy4 112.3(10) . . . . ?
O13 Dy2 Dy3 Dy4 -105.0(6) . . . . ?
O1 Dy2 Dy3 Dy4 178.5(7) 2_655 . . . ?
O14 Dy2 Dy3 Dy4 99.0(7) 4_646 . . . ?
O2W Dy2 Dy3 Dy4 -105(5) . . . . ?
O2 Dy2 Dy3 Dy4 -25.9(8) 3_456 . . . ?
O20 Dy2 Dy3 Dy4 -38.4(9) . . . . ?
O18 Dy2 Dy3 Dy4 36.6(4) . . . . ?
Dy1 Dy2 Dy3 Dy4 72.82(4) . . . . ?
O17 Dy2 Dy3 Dy1 39.5(9) . . . . ?
O13 Dy2 Dy3 Dy1 -177.8(6) . . . . ?
O1 Dy2 Dy3 Dy1 105.7(7) 2_655 . . . ?
O14 Dy2 Dy3 Dy1 26.1(7) 4_646 . . . ?
O2W Dy2 Dy3 Dy1 -177(5) . . . . ?
O2 Dy2 Dy3 Dy1 -98.7(8) 3_456 . . . ?
O20 Dy2 Dy3 Dy1 -111.2(9) . . . . ?
O18 Dy2 Dy3 Dy1 -36.2(4) . . . . ?
Dy4 Dy2 Dy3 Dy1 -72.82(4) . . . . ?
O7 Dy3 Dy4 O5 -56(5) 4_746 . . 3_456 ?
O19 Dy3 Dy4 O5 33(5) . . . 3_456 ?
O12 Dy3 Dy4 O5 -146(5) . . . 3_456 ?
O8 Dy3 Dy4 O5 132(5) . . . 3_456 ?
O20 Dy3 Dy4 O5 -113(5) . . . 3_456 ?
O9 Dy3 Dy4 O5 58(5) 4_746 . . 3_456 ?
O17 Dy3 Dy4 O5 -41(5) . . . 3_456 ?
O3W Dy3 Dy4 O5 138(5) . . . 3_456 ?
Dy1 Dy3 Dy4 O5 -3(5) . . . 3_456 ?
Dy2 Dy3 Dy4 O5 -73(5) . . . 3_456 ?
O7 Dy3 Dy4 O20 56.9(17) 4_746 . . . ?
O19 Dy3 Dy4 O20 146.0(12) . . . . ?
O12 Dy3 Dy4 O20 -33.3(11) . . . . ?
O8 Dy3 Dy4 O20 -114.9(12) . . . . ?
O9 Dy3 Dy4 O20 170.7(12) 4_746 . . . ?
O17 Dy3 Dy4 O20 72.2(11) . . . . ?
O3W Dy3 Dy4 O20 -109.4(13) . . . . ?
Dy1 Dy3 Dy4 O20 110.0(9) . . . . ?
Dy2 Dy3 Dy4 O20 40.0(9) . . . . ?
O7 Dy3 Dy4 O18 -22.0(15) 4_746 . . . ?
O19 Dy3 Dy4 O18 67.0(9) . . . . ?
O12 Dy3 Dy4 O18 -112.3(8) . . . . ?
O8 Dy3 Dy4 O18 166.2(9) . . . . ?
O20 Dy3 Dy4 O18 -78.9(10) . . . . ?
O9 Dy3 Dy4 O18 91.7(9) 4_746 . . . ?
O17 Dy3 Dy4 O18 -6.8(8) . . . . ?
O3W Dy3 Dy4 O18 171.7(10) . . . . ?
Dy1 Dy3 Dy4 O18 31.1(5) . . . . ?
Dy2 Dy3 Dy4 O18 -38.9(5) . . . . ?
O7 Dy3 Dy4 O19 -89.1(16) 4_746 . . . ?
O12 Dy3 Dy4 O19 -179.3(10) . . . . ?
O8 Dy3 Dy4 O19 99.2(10) . . . . ?
O20 Dy3 Dy4 O19 -146.0(12) . . . . ?
O9 Dy3 Dy4 O19 24.7(10) 4_746 . . . ?
O17 Dy3 Dy4 O19 -73.8(9) . . . . ?
O3W Dy3 Dy4 O19 104.7(12) . . . . ?
Dy1 Dy3 Dy4 O19 -36.0(8) . . . . ?
Dy2 Dy3 Dy4 O19 -106.0(8) . . . . ?
O7 Dy3 Dy4 O4 -132.1(15) 4_746 . . . ?
O19 Dy3 Dy4 O4 -43.0(9) . . . . ?
O12 Dy3 Dy4 O4 137.6(8) . . . . ?
O8 Dy3 Dy4 O4 56.1(9) . . . . ?
O20 Dy3 Dy4 O4 171.0(11) . . . . ?
O9 Dy3 Dy4 O4 -18.3(8) 4_746 . . . ?
O17 Dy3 Dy4 O4 -116.8(8) . . . . ?
O3W Dy3 Dy4 O4 61.6(10) . . . . ?
Dy1 Dy3 Dy4 O4 -79.0(5) . . . . ?
Dy2 Dy3 Dy4 O4 -149.0(5) . . . . ?
O7 Dy3 Dy4 O6 151.2(16) 4_746 . . . ?
O19 Dy3 Dy4 O6 -119.7(10) . . . . ?
O12 Dy3 Dy4 O6 61.0(10) . . . . ?
O8 Dy3 Dy4 O6 -20.6(10) . . . . ?
O20 Dy3 Dy4 O6 94.3(12) . . . . ?
O9 Dy3 Dy4 O6 -95.0(10) 4_746 . . . ?
O17 Dy3 Dy4 O6 166.5(9) . . . . ?
O3W Dy3 Dy4 O6 -15.1(11) . . . . ?
Dy1 Dy3 Dy4 O6 -155.7(7) . . . . ?
Dy2 Dy3 Dy4 O6 134.3(7) . . . . ?
O7 Dy3 Dy4 O3 81.5(15) 4_746 . . 3_456 ?
O19 Dy3 Dy4 O3 170.6(10) . . . 3_456 ?
O12 Dy3 Dy4 O3 -8.7(9) . . . 3_456 ?
O8 Dy3 Dy4 O3 -90.3(10) . . . 3_456 ?
O20 Dy3 Dy4 O3 24.6(11) . . . 3_456 ?
O9 Dy3 Dy4 O3 -164.7(9) 4_746 . . 3_456 ?
O17 Dy3 Dy4 O3 96.8(8) . . . 3_456 ?
O3W Dy3 Dy4 O3 -84.8(11) . . . 3_456 ?
Dy1 Dy3 Dy4 O3 134.6(6) . . . 3_456 ?
Dy2 Dy3 Dy4 O3 64.6(6) . . . 3_456 ?
O7 Dy3 Dy4 Dy2 16.9(14) 4_746 . . . ?
O19 Dy3 Dy4 Dy2 106.0(8) . . . . ?
O12 Dy3 Dy4 Dy2 -73.3(6) . . . . ?
O8 Dy3 Dy4 Dy2 -154.9(8) . . . . ?
O20 Dy3 Dy4 Dy2 -40.0(9) . . . . ?
O9 Dy3 Dy4 Dy2 130.7(7) 4_746 . . . ?
O17 Dy3 Dy4 Dy2 32.2(6) . . . . ?
O3W Dy3 Dy4 Dy2 -149.4(9) . . . . ?
Dy1 Dy3 Dy4 Dy2 70.02(4) . . . . ?
O7 Dy3 Dy4 Dy1 -53.1(14) 4_746 . . . ?
O19 Dy3 Dy4 Dy1 36.0(8) . . . . ?
O12 Dy3 Dy4 Dy1 -143.4(6) . . . . ?
O8 Dy3 Dy4 Dy1 135.1(8) . . . . ?
O20 Dy3 Dy4 Dy1 -110.0(9) . . . . ?
O9 Dy3 Dy4 Dy1 60.7(7) 4_746 . . . ?
O17 Dy3 Dy4 Dy1 -37.8(6) . . . . ?
O3W Dy3 Dy4 Dy1 140.6(9) . . . . ?
Dy2 Dy3 Dy4 Dy1 -70.02(4) . . . . ?
O17 Dy2 Dy4 O5 137.3(11) . . . 3_456 ?
O13 Dy2 Dy4 O5 -114.8(11) . . . 3_456 ?
O1 Dy2 Dy4 O5 166(2) 2_655 . . 3_456 ?
O14 Dy2 Dy4 O5 62.1(11) 4_646 . . 3_456 ?
O2W Dy2 Dy4 O5 -19.9(15) . . . 3_456 ?
O2 Dy2 Dy4 O5 -38.3(12) 3_456 . . 3_456 ?
O20 Dy2 Dy4 O5 -151.9(14) . . . 3_456 ?
O18 Dy2 Dy4 O5 63.8(12) . . . 3_456 ?
Dy1 Dy2 Dy4 O5 101.1(9) . . . 3_456 ?
Dy3 Dy2 Dy4 O5 170.4(9) . . . 3_456 ?
O17 Dy2 Dy4 O20 -70.8(11) . . . . ?
O13 Dy2 Dy4 O20 37.1(11) . . . . ?
O1 Dy2 Dy4 O20 -42(2) 2_655 . . . ?
O14 Dy2 Dy4 O20 -146.0(12) 4_646 . . . ?
O2W Dy2 Dy4 O20 132.0(15) . . . . ?
O2 Dy2 Dy4 O20 113.6(12) 3_456 . . . ?
O18 Dy2 Dy4 O20 -144.3(12) . . . . ?
Dy1 Dy2 Dy4 O20 -107.0(10) . . . . ?
Dy3 Dy2 Dy4 O20 -37.8(10) . . . . ?
O17 Dy2 Dy4 O18 73.5(9) . . . . ?
O13 Dy2 Dy4 O18 -178.6(9) . . . . ?
O1 Dy2 Dy4 O18 103(2) 2_655 . . . ?
O14 Dy2 Dy4 O18 -1.7(10) 4_646 . . . ?
O2W Dy2 Dy4 O18 -83.7(13) . . . . ?
O2 Dy2 Dy4 O18 -102.2(11) 3_456 . . . ?
O20 Dy2 Dy4 O18 144.3(12) . . . . ?
Dy1 Dy2 Dy4 O18 37.3(7) . . . . ?
Dy3 Dy2 Dy4 O18 106.5(7) . . . . ?
O17 Dy2 Dy4 O19 2.9(7) . . . . ?
O13 Dy2 Dy4 O19 110.8(8) . . . . ?
O1 Dy2 Dy4 O19 32(2) 2_655 . . . ?
O14 Dy2 Dy4 O19 -72.3(8) 4_646 . . . ?
O2W Dy2 Dy4 O19 -154.3(12) . . . . ?
O2 Dy2 Dy4 O19 -172.8(9) 3_456 . . . ?
O20 Dy2 Dy4 O19 73.7(11) . . . . ?
O18 Dy2 Dy4 O19 -70.6(9) . . . . ?
Dy1 Dy2 Dy4 O19 -33.3(5) . . . . ?
Dy3 Dy2 Dy4 O19 35.9(5) . . . . ?
O17 Dy2 Dy4 O4 28.0(11) . . . . ?
O13 Dy2 Dy4 O4 135.9(11) . . . . ?
O1 Dy2 Dy4 O4 57(2) 2_655 . . . ?
O14 Dy2 Dy4 O4 -47.2(11) 4_646 . . . ?
O2W Dy2 Dy4 O4 -129.2(15) . . . . ?
O2 Dy2 Dy4 O4 -147.7(12) 3_456 . . . ?
O20 Dy2 Dy4 O4 98.8(13) . . . . ?
O18 Dy2 Dy4 O4 -45.5(12) . . . . ?
Dy1 Dy2 Dy4 O4 -8.3(9) . . . . ?
Dy3 Dy2 Dy4 O4 61.0(9) . . . . ?
O17 Dy2 Dy4 O6 -87.1(8) . . . . ?
O13 Dy2 Dy4 O6 20.8(9) . . . . ?
O1 Dy2 Dy4 O6 -58(2) 2_655 . . . ?
O14 Dy2 Dy4 O6 -162.3(9) 4_646 . . . ?
O2W Dy2 Dy4 O6 115.7(13) . . . . ?
O2 Dy2 Dy4 O6 97.3(10) 3_456 . . . ?
O20 Dy2 Dy4 O6 -16.3(11) . . . . ?
O18 Dy2 Dy4 O6 -160.6(10) . . . . ?
Dy1 Dy2 Dy4 O6 -123.3(6) . . . . ?
Dy3 Dy2 Dy4 O6 -54.1(6) . . . . ?
O17 Dy2 Dy4 O3 -154.4(7) . . . 3_456 ?
O13 Dy2 Dy4 O3 -46.4(8) . . . 3_456 ?
O1 Dy2 Dy4 O3 -125(2) 2_655 . . 3_456 ?
O14 Dy2 Dy4 O3 130.5(8) 4_646 . . 3_456 ?
O2W Dy2 Dy4 O3 48.5(12) . . . 3_456 ?
O2 Dy2 Dy4 O3 30.0(9) 3_456 . . 3_456 ?
O20 Dy2 Dy4 O3 -83.6(11) . . . 3_456 ?
O18 Dy2 Dy4 O3 132.2(9) . . . 3_456 ?
Dy1 Dy2 Dy4 O3 169.4(5) . . . 3_456 ?
Dy3 Dy2 Dy4 O3 -121.3(5) . . . 3_456 ?
O17 Dy2 Dy4 Dy3 -33.1(5) . . . . ?
O13 Dy2 Dy4 Dy3 74.9(6) . . . . ?
O1 Dy2 Dy4 Dy3 -4.0(19) 2_655 . . . ?
O14 Dy2 Dy4 Dy3 -108.2(6) 4_646 . . . ?
O2W Dy2 Dy4 Dy3 169.8(11) . . . . ?
O2 Dy2 Dy4 Dy3 151.3(8) 3_456 . . . ?
O20 Dy2 Dy4 Dy3 37.8(10) . . . . ?
O18 Dy2 Dy4 Dy3 -106.5(7) . . . . ?
Dy1 Dy2 Dy4 Dy3 -69.25(4) . . . . ?
O17 Dy2 Dy4 Dy1 36.2(5) . . . . ?
O13 Dy2 Dy4 Dy1 144.1(6) . . . . ?
O1 Dy2 Dy4 Dy1 65.3(19) 2_655 . . . ?
O14 Dy2 Dy4 Dy1 -39.0(6) 4_646 . . . ?
O2W Dy2 Dy4 Dy1 -121.0(11) . . . . ?
O2 Dy2 Dy4 Dy1 -139.4(8) 3_456 . . . ?
O20 Dy2 Dy4 Dy1 107.0(10) . . . . ?
O18 Dy2 Dy4 Dy1 -37.3(7) . . . . ?
Dy3 Dy2 Dy4 Dy1 69.25(4) . . . . ?
O16 Dy1 Dy4 O5 -91.6(11) 4_646 . . 3_456 ?
O15 Dy1 Dy4 O5 65.1(10) 2_654 . . 3_456 ?
O11 Dy1 Dy4 O5 -10.4(10) 2_654 . . 3_456 ?
O18 Dy1 Dy4 O5 -64.0(11) . . . 3_456 ?
O19 Dy1 Dy4 O5 141.9(12) . . . 3_456 ?
O10 Dy1 Dy4 O5 158.6(10) 4_746 . . 3_456 ?
O17 Dy1 Dy4 O5 -142.7(10) . . . 3_456 ?
O1W Dy1 Dy4 O5 58.0(15) . . . 3_456 ?
Dy3 Dy1 Dy4 O5 179.5(8) . . . 3_456 ?
Dy2 Dy1 Dy4 O5 -107.4(8) . . . 3_456 ?
O16 Dy1 Dy4 O20 53.8(10) 4_646 . . . ?
O15 Dy1 Dy4 O20 -149.5(8) 2_654 . . . ?
O11 Dy1 Dy4 O20 135.0(9) 2_654 . . . ?
O18 Dy1 Dy4 O20 81.4(10) . . . . ?
O19 Dy1 Dy4 O20 -72.7(11) . . . . ?
O10 Dy1 Dy4 O20 -56.0(8) 4_746 . . . ?
O17 Dy1 Dy4 O20 2.7(9) . . . . ?
O1W Dy1 Dy4 O20 -156.7(15) . . . . ?
Dy3 Dy1 Dy4 O20 -35.1(6) . . . . ?
Dy2 Dy1 Dy4 O20 38.0(6) . . . . ?
O16 Dy1 Dy4 O18 -27.7(12) 4_646 . . . ?
O15 Dy1 Dy4 O18 129.0(10) 2_654 . . . ?
O11 Dy1 Dy4 O18 53.5(10) 2_654 . . . ?
O19 Dy1 Dy4 O18 -154.2(12) . . . . ?
O10 Dy1 Dy4 O18 -137.5(10) 4_746 . . . ?
O17 Dy1 Dy4 O18 -78.7(10) . . . . ?
O1W Dy1 Dy4 O18 121.9(16) . . . . ?
Dy3 Dy1 Dy4 O18 -116.6(8) . . . . ?
Dy2 Dy1 Dy4 O18 -43.5(8) . . . . ?
O16 Dy1 Dy4 O19 126.5(12) 4_646 . . . ?
O15 Dy1 Dy4 O19 -76.8(11) 2_654 . . . ?
O11 Dy1 Dy4 O19 -152.3(11) 2_654 . . . ?
O18 Dy1 Dy4 O19 154.2(12) . . . . ?
O10 Dy1 Dy4 O19 16.7(11) 4_746 . . . ?
O17 Dy1 Dy4 O19 75.5(11) . . . . ?
O1W Dy1 Dy4 O19 -83.9(16) . . . . ?
Dy3 Dy1 Dy4 O19 37.6(9) . . . . ?
Dy2 Dy1 Dy4 O19 110.7(9) . . . . ?
O16 Dy1 Dy4 O4 -169.0(9) 4_646 . . . ?
O15 Dy1 Dy4 O4 -12.3(8) 2_654 . . . ?
O11 Dy1 Dy4 O4 -87.8(8) 2_654 . . . ?
O18 Dy1 Dy4 O4 -141.3(10) . . . . ?
O19 Dy1 Dy4 O4 64.5(10) . . . . ?
O10 Dy1 Dy4 O4 81.2(8) 4_746 . . . ?
O17 Dy1 Dy4 O4 139.9(8) . . . . ?
O1W Dy1 Dy4 O4 -19.4(14) . . . . ?
Dy3 Dy1 Dy4 O4 102.1(6) . . . . ?
Dy2 Dy1 Dy4 O4 175.2(6) . . . . ?
O16 Dy1 Dy4 O6 121.4(12) 4_646 . . . ?
O15 Dy1 Dy4 O6 -81.9(12) 2_654 . . . ?
O11 Dy1 Dy4 O6 -157.4(12) 2_654 . . . ?
O18 Dy1 Dy4 O6 149.0(13) . . . . ?
O19 Dy1 Dy4 O6 -5.1(14) . . . . ?
O10 Dy1 Dy4 O6 11.6(11) 4_746 . . . ?
O17 Dy1 Dy4 O6 70.3(12) . . . . ?
O1W Dy1 Dy4 O6 -89.0(17) . . . . ?
Dy3 Dy1 Dy4 O6 32.5(10) . . . . ?
Dy2 Dy1 Dy4 O6 105.6(10) . . . . ?
O16 Dy1 Dy4 O3 0.0(11) 4_646 . . 3_456 ?
O15 Dy1 Dy4 O3 156.7(9) 2_654 . . 3_456 ?
O11 Dy1 Dy4 O3 81.2(10) 2_654 . . 3_456 ?
O18 Dy1 Dy4 O3 27.7(11) . . . 3_456 ?
O19 Dy1 Dy4 O3 -126.5(12) . . . 3_456 ?
O10 Dy1 Dy4 O3 -109.8(10) 4_746 . . 3_456 ?
O17 Dy1 Dy4 O3 -51.0(10) . . . 3_456 ?
O1W Dy1 Dy4 O3 149.6(15) . . . 3_456 ?
Dy3 Dy1 Dy4 O3 -88.9(8) . . . 3_456 ?
Dy2 Dy1 Dy4 O3 -15.8(8) . . . 3_456 ?
O16 Dy1 Dy4 Dy3 88.9(8) 4_646 . . . ?
O15 Dy1 Dy4 Dy3 -114.4(5) 2_654 . . . ?
O11 Dy1 Dy4 Dy3 170.1(6) 2_654 . . . ?
O18 Dy1 Dy4 Dy3 116.6(8) . . . . ?
O19 Dy1 Dy4 Dy3 -37.6(9) . . . . ?
O10 Dy1 Dy4 Dy3 -20.9(6) 4_746 . . . ?
O17 Dy1 Dy4 Dy3 37.9(6) . . . . ?
O1W Dy1 Dy4 Dy3 -121.5(13) . . . . ?
Dy2 Dy1 Dy4 Dy3 73.09(4) . . . . ?
O16 Dy1 Dy4 Dy2 15.8(8) 4_646 . . . ?
O15 Dy1 Dy4 Dy2 172.5(6) 2_654 . . . ?
O11 Dy1 Dy4 Dy2 97.0(6) 2_654 . . . ?
O18 Dy1 Dy4 Dy2 43.5(8) . . . . ?
O19 Dy1 Dy4 Dy2 -110.7(9) . . . . ?
O10 Dy1 Dy4 Dy2 -94.0(6) 4_746 . . . ?
O17 Dy1 Dy4 Dy2 -35.2(6) . . . . ?
O1W Dy1 Dy4 Dy2 165.4(13) . . . . ?
Dy3 Dy1 Dy4 Dy2 -73.09(4) . . . . ?
O5 Dy4 O4 S1 56(3) 3_456 . . . ?
O20 Dy4 O4 S1 -125(2) . . . . ?
O18 Dy4 O4 S1 147(2) . . . . ?
O19 Dy4 O4 S1 -158(3) . . . . ?
O6 Dy4 O4 S1 -57(3) . . . . ?
O3 Dy4 O4 S1 0(3) 3_456 . . . ?
Dy3 Dy4 O4 S1 -133(2) . . . . ?
Dy2 Dy4 O4 S1 176.3(18) . . . . ?
Dy1 Dy4 O4 S1 169(3) . . . . ?
O5 Dy4 O6 S2 -148(2) 3_456 . . . ?
O20 Dy4 O6 S2 65(2) . . . . ?
O18 Dy4 O6 S2 44(3) . . . . ?
O19 Dy4 O6 S2 -4(2) . . . . ?
O4 Dy4 O6 S2 -73(2) . . . . ?
O3 Dy4 O6 S2 144(2) 3_456 . . . ?
Dy3 Dy4 O6 S2 27.7(19) . . . . ?
Dy2 Dy4 O6 S2 75(2) . . . . ?
Dy1 Dy4 O6 S2 -1(3) . . . . ?
O7 Dy3 O8 S2 -130(3) 4_746 . . . ?
O19 Dy3 O8 S2 78(3) . . . . ?
O12 Dy3 O8 S2 -64(3) . . . . ?
O20 Dy3 O8 S2 9(3) . . . . ?
O9 Dy3 O8 S2 157(3) 4_746 . . . ?
O17 Dy3 O8 S2 51(4) . . . . ?
O3W Dy3 O8 S2 -135(3) . . . . ?
Dy4 Dy3 O8 S2 41(3) . . . . ?
Dy1 Dy3 O8 S2 82(3) . . . . ?
Dy2 Dy3 O8 S2 16(3) . . . . ?
O7 Dy3 O12 S3 125(3) 4_746 . . . ?
O19 Dy3 O12 S3 -91(3) . . . . ?
O8 Dy3 O12 S3 -27(3) . . . . ?
O20 Dy3 O12 S3 -110(3) . . . . ?
O9 Dy3 O12 S3 54(4) 4_746 . . . ?
O17 Dy3 O12 S3 -169(3) . . . . ?
O3W Dy3 O12 S3 46(3) . . . . ?
Dy4 Dy3 O12 S3 -90(3) . . . . ?
Dy1 Dy3 O12 S3 -149(2) . . . . ?
Dy2 Dy3 O12 S3 -146(3) . . . . ?
O17 Dy2 O13 S4 -126(3) . . . . ?
O1 Dy2 O13 S4 -46(3) 2_655 . . . ?
O14 Dy2 O13 S4 -18(4) 4_646 . . . ?
O2W Dy2 O13 S4 32(3) . . . . ?
O2 Dy2 O13 S4 99(3) 3_456 . . . ?
O20 Dy2 O13 S4 178(3) . . . . ?
O18 Dy2 O13 S4 154(2) . . . . ?
Dy4 Dy2 O13 S4 156(3) . . . . ?
Dy1 Dy2 O13 S4 -151(2) . . . . ?
Dy3 Dy2 O13 S4 -148(3) . . . . ?
O13 Dy2 O17 Dy3 -39.4(11) . . . . ?
O1 Dy2 O17 Dy3 -114.9(11) 2_655 . . . ?
O14 Dy2 O17 Dy3 167.8(11) 4_646 . . . ?
O2W Dy2 O17 Dy3 -168.8(16) . . . . ?
O2 Dy2 O17 Dy3 59.8(14) 3_456 . . . ?
O20 Dy2 O17 Dy3 17.8(8) . . . . ?
O18 Dy2 O17 Dy3 92.6(9) . . . . ?
Dy4 Dy2 O17 Dy3 54.6(7) . . . . ?
Dy1 Dy2 O17 Dy3 114.4(13) . . . . ?
O13 Dy2 O17 Dy1 -153.8(8) . . . . ?
O1 Dy2 O17 Dy1 130.7(10) 2_655 . . . ?
O14 Dy2 O17 Dy1 53.4(9) 4_646 . . . ?
O2W Dy2 O17 Dy1 77(2) . . . . ?
O2 Dy2 O17 Dy1 -54.6(14) 3_456 . . . ?
O20 Dy2 O17 Dy1 -96.6(10) . . . . ?
O18 Dy2 O17 Dy1 -21.8(7) . . . . ?
Dy4 Dy2 O17 Dy1 -59.8(7) . . . . ?
Dy3 Dy2 O17 Dy1 -114.4(13) . . . . ?
O7 Dy3 O17 Dy2 116.0(13) 4_746 . . . ?
O19 Dy3 O17 Dy2 -92.3(10) . . . . ?
O12 Dy3 O17 Dy2 43.5(11) . . . . ?
O8 Dy3 O17 Dy2 -64.9(17) . . . . ?
O20 Dy3 O17 Dy2 -18.4(8) . . . . ?
O9 Dy3 O17 Dy2 -164.0(10) 4_746 . . . ?
O3W Dy3 O17 Dy2 127.0(13) . . . . ?
Dy4 Dy3 O17 Dy2 -54.9(7) . . . . ?
Dy1 Dy3 O17 Dy2 -116.4(12) . . . . ?
O7 Dy3 O17 Dy1 -127.6(12) 4_746 . . . ?
O19 Dy3 O17 Dy1 24.1(7) . . . . ?
O12 Dy3 O17 Dy1 159.9(9) . . . . ?
O8 Dy3 O17 Dy1 51.5(16) . . . . ?
O20 Dy3 O17 Dy1 98.0(9) . . . . ?
O9 Dy3 O17 Dy1 -47.6(9) 4_746 . . . ?
O3W Dy3 O17 Dy1 -116.6(14) . . . . ?
Dy4 Dy3 O17 Dy1 61.5(6) . . . . ?
Dy2 Dy3 O17 Dy1 116.4(12) . . . . ?
O16 Dy1 O17 Dy2 -85.1(10) 4_646 . . . ?
O15 Dy1 O17 Dy2 106.7(13) 2_654 . . . ?
O11 Dy1 O17 Dy2 -22.6(14) 2_654 . . . ?
O18 Dy1 O17 Dy2 23.0(7) . . . . ?
O19 Dy1 O17 Dy2 94.6(10) . . . . ?
O10 Dy1 O17 Dy2 -177.0(11) 4_746 . . . ?
O1W Dy1 O17 Dy2 -132.5(9) . . . . ?
Dy3 Dy1 O17 Dy2 118.6(11) . . . . ?
Dy4 Dy1 O17 Dy2 58.7(6) . . . . ?
O16 Dy1 O17 Dy3 156.3(10) 4_646 . . . ?
O15 Dy1 O17 Dy3 -11.8(16) 2_654 . . . ?
O11 Dy1 O17 Dy3 -141.2(10) 2_654 . . . ?
O18 Dy1 O17 Dy3 -95.5(8) . . . . ?
O19 Dy1 O17 Dy3 -24.0(7) . . . . ?
O10 Dy1 O17 Dy3 64.5(9) 4_746 . . . ?
O1W Dy1 O17 Dy3 108.9(10) . . . . ?
Dy2 Dy1 O17 Dy3 -118.6(11) . . . . ?
Dy4 Dy1 O17 Dy3 -59.9(6) . . . . ?
O5 Dy4 O18 Dy1 122.9(10) 3_456 . . . ?
O20 Dy4 O18 Dy1 -89.4(10) . . . . ?
O19 Dy4 O18 Dy1 -15.7(8) . . . . ?
O4 Dy4 O18 Dy1 41.8(11) . . . . ?
O6 Dy4 O18 Dy1 -68(2) . . . . ?
O3 Dy4 O18 Dy1 -161.3(8) 3_456 . . . ?
Dy3 Dy4 O18 Dy1 -52.0(6) . . . . ?
Dy2 Dy4 O18 Dy1 -111.7(11) . . . . ?
O5 Dy4 O18 Dy2 -125.4(10) 3_456 . . . ?
O20 Dy4 O18 Dy2 22.3(8) . . . . ?
O19 Dy4 O18 Dy2 96.1(8) . . . . ?
O4 Dy4 O18 Dy2 153.5(7) . . . . ?
O6 Dy4 O18 Dy2 44(2) . . . . ?
O3 Dy4 O18 Dy2 -49.5(9) 3_456 . . . ?
Dy3 Dy4 O18 Dy2 59.8(5) . . . . ?
Dy1 Dy4 O18 Dy2 111.7(11) . . . . ?
O16 Dy1 O18 Dy4 159.6(9) 4_646 . . . ?
O15 Dy1 O18 Dy4 -51.4(10) 2_654 . . . ?
O11 Dy1 O18 Dy4 -123.8(10) 2_654 . . . ?
O19 Dy1 O18 Dy4 15.5(8) . . . . ?
O10 Dy1 O18 Dy4 62.2(13) 4_746 . . . ?
O17 Dy1 O18 Dy4 89.8(9) . . . . ?
O1W Dy1 O18 Dy4 -131.6(13) . . . . ?
Dy3 Dy1 O18 Dy4 51.6(6) . . . . ?
Dy2 Dy1 O18 Dy4 110.9(10) . . . . ?
O16 Dy1 O18 Dy2 48.8(8) 4_646 . . . ?
O15 Dy1 O18 Dy2 -162.3(7) 2_654 . . . ?
O11 Dy1 O18 Dy2 125.4(9) 2_654 . . . ?
O19 Dy1 O18 Dy2 -95.3(8) . . . . ?
O10 Dy1 O18 Dy2 -48.7(12) 4_746 . . . ?
O17 Dy1 O18 Dy2 -21.0(7) . . . . ?
O1W Dy1 O18 Dy2 117.6(14) . . . . ?
Dy3 Dy1 O18 Dy2 -59.3(5) . . . . ?
Dy4 Dy1 O18 Dy2 -110.9(10) . . . . ?
O17 Dy2 O18 Dy4 -94.8(8) . . . . ?
O13 Dy2 O18 Dy4 2.0(13) . . . . ?
O1 Dy2 O18 Dy4 -143.5(11) 2_655 . . . ?
O14 Dy2 O18 Dy4 178.3(9) 4_646 . . . ?
O2W Dy2 O18 Dy4 115.6(11) . . . . ?
O2 Dy2 O18 Dy4 61.0(9) 3_456 . . . ?
O20 Dy2 O18 Dy4 -21.6(7) . . . . ?
Dy1 Dy2 O18 Dy4 -116.8(10) . . . . ?
Dy3 Dy2 O18 Dy4 -58.4(5) . . . . ?
O17 Dy2 O18 Dy1 22.0(7) . . . . ?
O13 Dy2 O18 Dy1 118.8(10) . . . . ?
O1 Dy2 O18 Dy1 -26.6(15) 2_655 . . . ?
O14 Dy2 O18 Dy1 -64.8(8) 4_646 . . . ?
O2W Dy2 O18 Dy1 -127.6(11) . . . . ?
O2 Dy2 O18 Dy1 177.8(10) 3_456 . . . ?
O20 Dy2 O18 Dy1 95.3(8) . . . . ?
Dy4 Dy2 O18 Dy1 116.8(10) . . . . ?
Dy3 Dy2 O18 Dy1 58.4(5) . . . . ?
O5 Dy4 O19 Dy3 -172.9(10) 3_456 . . . ?
O20 Dy4 O19 Dy3 -20.9(7) . . . . ?
O18 Dy4 O19 Dy3 -101.9(9) . . . . ?
O4 Dy4 O19 Dy3 134.3(9) . . . . ?
O6 Dy4 O19 Dy3 58.7(10) . . . . ?
O3 Dy4 O19 Dy3 -16.3(17) 3_456 . . . ?
Dy2 Dy4 O19 Dy3 -60.8(6) . . . . ?
Dy1 Dy4 O19 Dy3 -117.4(11) . . . . ?
O5 Dy4 O19 Dy1 -55.5(15) 3_456 . . . ?
O20 Dy4 O19 Dy1 96.5(10) . . . . ?
O18 Dy4 O19 Dy1 15.5(7) . . . . ?
O4 Dy4 O19 Dy1 -108.3(10) . . . . ?
O6 Dy4 O19 Dy1 176.1(10) . . . . ?
O3 Dy4 O19 Dy1 101.1(14) 3_456 . . . ?
Dy3 Dy4 O19 Dy1 117.4(11) . . . . ?
Dy2 Dy4 O19 Dy1 56.6(7) . . . . ?
O7 Dy3 O19 Dy4 131.2(13) 4_746 . . . ?
O12 Dy3 O19 Dy4 1.0(15) . . . . ?
O8 Dy3 O19 Dy4 -67.8(9) . . . . ?
O20 Dy3 O19 Dy4 20.5(7) . . . . ?
O9 Dy3 O19 Dy4 -156.6(10) 4_746 . . . ?
O17 Dy3 O19 Dy4 94.5(8) . . . . ?
O3W Dy3 O19 Dy4 -114.2(10) . . . . ?
Dy1 Dy3 O19 Dy4 119.5(11) . . . . ?
Dy2 Dy3 O19 Dy4 59.1(6) . . . . ?
O7 Dy3 O19 Dy1 11.7(17) 4_746 . . . ?
O12 Dy3 O19 Dy1 -118.5(12) . . . . ?
O8 Dy3 O19 Dy1 172.7(11) . . . . ?
O20 Dy3 O19 Dy1 -99.0(10) . . . . ?
O9 Dy3 O19 Dy1 83.9(11) 4_746 . . . ?
O17 Dy3 O19 Dy1 -25.0(8) . . . . ?
O3W Dy3 O19 Dy1 126.2(9) . . . . ?
Dy4 Dy3 O19 Dy1 -119.5(11) . . . . ?
Dy2 Dy3 O19 Dy1 -60.4(6) . . . . ?
O16 Dy1 O19 Dy4 -91.9(16) 4_646 . . . ?
O15 Dy1 O19 Dy4 95.3(10) 2_654 . . . ?
O11 Dy1 O19 Dy4 34.1(13) 2_654 . . . ?
O18 Dy1 O19 Dy4 -15.4(7) . . . . ?
O10 Dy1 O19 Dy4 -164.7(10) 4_746 . . . ?
O17 Dy1 O19 Dy4 -92.4(9) . . . . ?
O1W Dy1 O19 Dy4 142.3(9) . . . . ?
Dy3 Dy1 O19 Dy4 -117.3(12) . . . . ?
Dy2 Dy1 O19 Dy4 -55.9(7) . . . . ?
O16 Dy1 O19 Dy3 25.3(18) 4_646 . . . ?
O15 Dy1 O19 Dy3 -147.4(10) 2_654 . . . ?
O11 Dy1 O19 Dy3 151.4(9) 2_654 . . . ?
O18 Dy1 O19 Dy3 101.9(9) . . . . ?
O10 Dy1 O19 Dy3 -47.4(9) 4_746 . . . ?
O17 Dy1 O19 Dy3 24.9(8) . . . . ?
O1W Dy1 O19 Dy3 -100.4(11) . . . . ?
Dy2 Dy1 O19 Dy3 61.4(6) . . . . ?
Dy4 Dy1 O19 Dy3 117.3(12) . . . . ?
O5 Dy4 O20 Dy3 164.9(15) 3_456 . . . ?
O18 Dy4 O20 Dy3 92.0(9) . . . . ?
O19 Dy4 O20 Dy3 20.8(7) . . . . ?
O4 Dy4 O20 Dy3 -12.4(14) . . . . ?
O6 Dy4 O20 Dy3 -79.2(10) . . . . ?
O3 Dy4 O20 Dy3 -156.7(10) 3_456 . . . ?
Dy2 Dy4 O20 Dy3 114.9(12) . . . . ?
Dy1 Dy4 O20 Dy3 56.4(7) . . . . ?
O5 Dy4 O20 Dy2 50(2) 3_456 . . . ?
O18 Dy4 O20 Dy2 -22.9(8) . . . . ?
O19 Dy4 O20 Dy2 -94.1(9) . . . . ?
O4 Dy4 O20 Dy2 -127.3(9) . . . . ?
O6 Dy4 O20 Dy2 165.8(10) . . . . ?
O3 Dy4 O20 Dy2 88.4(9) 3_456 . . . ?
Dy3 Dy4 O20 Dy2 -114.9(12) . . . . ?
Dy1 Dy4 O20 Dy2 -58.5(7) . . . . ?
O7 Dy3 O20 Dy4 -147.0(10) 4_746 . . . ?
O19 Dy3 O20 Dy4 -20.9(8) . . . . ?
O12 Dy3 O20 Dy4 145.7(12) . . . . ?
O8 Dy3 O20 Dy4 56.0(10) . . . . ?
O9 Dy3 O20 Dy4 -16(2) 4_746 . . . ?
O17 Dy3 O20 Dy4 -96.2(10) . . . . ?
O3W Dy3 O20 Dy4 110.8(11) . . . . ?
Dy1 Dy3 O20 Dy4 -57.7(7) . . . . ?
Dy2 Dy3 O20 Dy4 -113.3(12) . . . . ?
O7 Dy3 O20 Dy2 -33.8(13) 4_746 . . . ?
O19 Dy3 O20 Dy2 92.4(9) . . . . ?
O12 Dy3 O20 Dy2 -101.0(11) . . . . ?
O8 Dy3 O20 Dy2 169.2(11) . . . . ?
O9 Dy3 O20 Dy2 97.6(16) 4_746 . . . ?
O17 Dy3 O20 Dy2 17.1(7) . . . . ?
O3W Dy3 O20 Dy2 -135.9(10) . . . . ?
Dy4 Dy3 O20 Dy2 113.3(12) . . . . ?
Dy1 Dy3 O20 Dy2 55.6(7) . . . . ?
O17 Dy2 O20 Dy4 97.4(10) . . . . ?
O13 Dy2 O20 Dy4 -140.4(11) . . . . ?
O1 Dy2 O20 Dy4 162.1(9) 2_655 . . . ?
O14 Dy2 O20 Dy4 50.7(15) 4_646 . . . ?
O2W Dy2 O20 Dy4 -77.7(16) . . . . ?
O2 Dy2 O20 Dy4 -53.0(10) 3_456 . . . ?
O18 Dy2 O20 Dy4 22.1(7) . . . . ?
Dy1 Dy2 O20 Dy4 59.6(7) . . . . ?
Dy3 Dy2 O20 Dy4 115.0(13) . . . . ?
O17 Dy2 O20 Dy3 -17.6(8) . . . . ?
O13 Dy2 O20 Dy3 104.5(10) . . . . ?
O1 Dy2 O20 Dy3 47.1(13) 2_655 . . . ?
O14 Dy2 O20 Dy3 -64.3(14) 4_646 . . . ?
O2W Dy2 O20 Dy3 167.2(13) . . . . ?
O2 Dy2 O20 Dy3 -168.0(11) 3_456 . . . ?
O18 Dy2 O20 Dy3 -93.0(9) . . . . ?
Dy4 Dy2 O20 Dy3 -115.0(13) . . . . ?
Dy1 Dy2 O20 Dy3 -55.4(7) . . . . ?
Dy2 O2 S1 O4 -177(3) 3_556 . . . ?
Dy2 O2 S1 O1 -56(4) 3_556 . . . ?
Dy2 O2 S1 O3 64(3) 3_556 . . . ?
Dy4 O4 S1 O2 -3(3) . . . . ?
Dy4 O4 S1 O1 -126(2) . . . . ?
Dy4 O4 S1 O3 113(3) . . . . ?
Dy2 O1 S1 O2 -102(10) 2_654 . . . ?
Dy2 O1 S1 O4 17(11) 2_654 . . . ?
Dy2 O1 S1 O3 139(10) 2_654 . . . ?
Dy4 O3 S1 O2 13.9(18) 3_556 . . . ?
Dy4 O3 S1 O4 -102.4(14) 3_556 . . . ?
Dy4 O3 S1 O1 135.9(14) 3_556 . . . ?
Dy3 O8 S2 O5 -154(3) . . . . ?
Dy3 O8 S2 O7 91(3) . . . . ?
Dy3 O8 S2 O6 -31(4) . . . . ?
Dy4 O5 S2 O8 150(4) 3_556 . . . ?
Dy4 O5 S2 O7 -92(4) 3_556 . . . ?
Dy4 O5 S2 O6 27(5) 3_556 . . . ?
Dy3 O7 S2 O8 -95(5) 4_756 . . . ?
Dy3 O7 S2 O5 147(5) 4_756 . . . ?
Dy3 O7 S2 O6 28(5) 4_756 . . . ?
Dy4 O6 S2 O8 -17(3) . . . . ?
Dy4 O6 S2 O5 105(2) . . . . ?
Dy4 O6 S2 O7 -139(2) . . . . ?
Dy1 O11 S3 O9 58(5) 2_655 . . . ?
Dy1 O11 S3 O12 -62(5) 2_655 . . . ?
Dy1 O11 S3 O10 180(4) 2_655 . . . ?
Dy3 O9 S3 O11 122.0(17) 4_756 . . . ?
Dy3 O9 S3 O12 -119.5(16) 4_756 . . . ?
Dy3 O9 S3 O10 0(2) 4_756 . . . ?
Dy3 O12 S3 O11 -150(3) . . . . ?
Dy3 O12 S3 O9 90(3) . . . . ?
Dy3 O12 S3 O10 -30(3) . . . . ?
Dy1 O10 S3 O11 -50(2) 4_756 . . . ?
Dy1 O10 S3 O9 72(2) 4_756 . . . ?
Dy1 O10 S3 O12 -167.6(17) 4_756 . . . ?
Dy2 O13 S4 O15 116(3) . . . . ?
Dy2 O13 S4 O16 -6(3) . . . . ?
Dy2 O13 S4 O14 -126(3) . . . . ?
Dy1 O15 S4 O13 140(4) 2_655 . . . ?
Dy1 O15 S4 O16 -98(4) 2_655 . . . ?
Dy1 O15 S4 O14 22(4) 2_655 . . . ?
Dy1 O16 S4 O13 -145.8(15) 4_656 . . . ?
Dy1 O16 S4 O15 94.2(18) 4_656 . . . ?
Dy1 O16 S4 O14 -26(2) 4_656 . . . ?
Dy2 O14 S4 O13 80(3) 4_656 . . . ?
Dy2 O14 S4 O15 -163(2) 4_656 . . . ?
Dy2 O14 S4 O16 -41(3) 4_656 . . . ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        25.01
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         6.994
_refine_diff_density_min         -5.386
_refine_diff_density_rms         0.903
_database_code_depnum_ccdc_archive 'CCDC 981570'
